"This text is intended to serve as an introduction to the science of microlithography, but also covers several subj
325 59 16MB
English Pages 630  Year 2019
798 170 231MB Read more
839 99 8MB Read more
"Preface to Fourth Edition Since publication of the first edition of Principles of Ecotoxicology, both David Peakal
970 149 7MB Read more
585 23 19MB Read more
775 92 11MB Read more
This book covers the many aspects of lithographic technology that needed to be addressed in order to make EUV lithograph
203 30 6MB Read more
766 128 19MB Read more
1,727 126 8MB Read more
Table of contents :
Preface to the Fourth Edition
Preface to the Third Edition
Preface to the Second Edition
Preface to the First Edition
Chapter 1 OVERVIEW OF LITHOGRAPHY
Chapter 2 OPTICAL PATTERN FORMATION
Chapter 3 PHOTORESISTS
Chapter 4 MODELING AND THIN-FILM EFFECTS
Chapter 5 WAFER STEPPERS AND SCANNERS
Chapter 6 OVERLAY
Chapter 7 MASKS AND RETICLES
Chapter 8 CONFRONTING THE DIFFRACTION LIMIT
Chapter 9 METROLOGY
Chapter 10 IMMERSION LITHOGRAPHY AND THE LIMITS OF OPTICAL LITHOGRAPHY
Chapter 11 LITHOGRAPHY COSTS
Chapter 12 EXTREME ULTRAVIOLET LITHOGRAPHY
Chapter 13 ALTERNATIVE LITHOGRAPHY TECHNIQUES
Appendix A COHERENCE
Principles of Lithography Fourth Edition
Principles of Lithography Fourth Edition
Harry J. Levinson
SPIE PRESS Bellingham, Washington USA
Library of Congress Cataloguing-in-Publication Data Names: Levinson, Harry J., author. Title: Principles of lithography / Harry J. Levinson. Description: Fourth edition. | Bellingham, Washington, USA : SPIE Press,  | Includes bibliographical references and index. Identifiers: LCCN 2019000488 (print) | LCCN 2019003004 (ebook) | ISBN 9781510627611 (pdf) | ISBN 9781510627628 (epub) | ISBN 9781510627635 (mobi) | ISBN 9781510627604 | ISBN 9781510627604¬(softcover) | ISBN 151062760X¬(softcover) Subjects: LCSH: Integrated circuits--Design and construction. | Microlithography. Classification: LCC TK7874 (ebook) | LCC TK7874 .L397 2019 (print) | DDC 621.3815/31--dc23 LC record available at https://lccn.loc.gov/2019000488
Published by SPIE P.O. Box 10 Bellingham, Washington 98227-0010 USA Phone: +1 360.676.3290 Fax: +1 360.647.1445 Email: [email protected] Web: http://spie.org Copyright © 2019 Society of Photo-Optical Instrumentation Engineers (SPIE) All rights reserved. No part of this publication may be reproduced or distributed in any form or by any means without written permission of the publisher. The content of this book reflects the work and thought of the author. Every effort has been made to publish reliable and accurate information herein, but the publisher is not responsible for the validity of the information or for any outcomes resulting from reliance thereon. Printed in the United States of America. First printing For updates to this book, visit http://spie.org and type “PM304” in the search field.
Contents Preface to the Fourth Edition ................................................................ ix Preface to the Third Edition................................................................... xi Preface to the Second Edition............................................................. xiii Preface to the First Edition ................................................................... xv Chapter 1
Overview of Lithography .................................................... 1
Problems ................................................................................................... 6 Chapter 2
Optical Pattern Formation................................................... 7
2.1 The Problem of Imaging ................................................................. 7 2.2 Aerial Images ................................................................................ 10 2.3 The Contributions of Physics and Chemistry................................ 23 2.4 Focus ............................................................................................. 33 Problems ................................................................................................. 49 References............................................................................................... 50 Chapter 3
Photoresists ...................................................................... 53
3.1 Positive and Negative Resists ....................................................... 53 3.2 Adhesion Promotion ..................................................................... 57 3.3 Resist Spin Coating, Softbake, and Hardbake .............................. 60 3.4 Photochemistry of Novolak/DNQ g- and i-line Resists ................ 72 3.5 Acid-Catalyzed DUV Resists........................................................ 75 3.6 Development and Post-Exposure Bakes ....................................... 81 3.7 Operational Characterization ........................................................ 86 3.8 Line-Edge Roughness ................................................................... 88 3.9 Multilayer Resist Processes ........................................................ 102 Problems ............................................................................................... 106 References............................................................................................. 106
Modeling and Thin-Film Effects .................................... 123
4.1 Models of Optical Imaging ......................................................... 124 4.2 Aberrations .................................................................................. 129 4.3 Modeling Photochemical Reactions ............................................ 138 4.4 Thin-Film Optical Effects ........................................................... 141 4.5 Post-Exposure Bakes................................................................... 147 4.6 Methods for Addressing the Problems of Reflective Substrates . 150 4.7 Development ............................................................................... 158 4.8 Quantum Effects and Modeling .................................................. 159 4.9 Summary of Modeling ................................................................ 162 Problems ............................................................................................... 162 References ............................................................................................. 163 Chapter 5
Wafer Steppers and Scanners ....................................... 169
5.1 Overview ..................................................................................... 169 5.2 Light Sources .............................................................................. 172 5.3 Illumination Systems................................................................... 185 5.4 Reduction Lenses ........................................................................ 190 5.5 Autofocus Systems ...................................................................... 207 5.6 The Wafer Stage.......................................................................... 209 5.7 Scanning ...................................................................................... 215 5.8 Dual-Stage Exposure Tools......................................................... 218 5.9 Lithography Exposure Tools before Steppers ............................. 219 Problems ............................................................................................... 224 References ............................................................................................. 225 Chapter 6
Overlay ............................................................................ 241
Alignment Systems ..................................................................... 243 6.1.1 Classification of alignment systems ............................... 247 6.1.2 Optical methods for alignment and wafer-to-reticle referencing ..................................................................... 247 6.1.3 Number of alignment marks .......................................... 253 6.2 Overlay Models ........................................................................... 255 6.3 Matching ..................................................................................... 266 6.4 Process-Dependent Overlay Effects ............................................ 277 Problems ............................................................................................... 279 References ............................................................................................. 281
Masks and Reticles ........................................................ 289
7.1 7.2 7.3 7.4
Overview ..................................................................................... 289 Mask Blanks ................................................................................ 290 Mechanical Optical-Pattern Generators ...................................... 292 Electron-Beam Lithography and Single-Beam Mask Writers .... 293
7.5 Multi-Electron-Beam Mask Writers ........................................... 308 7.6 Optical Mask Writers .................................................................. 310 7.7 Resists for Mask Making ............................................................ 312 7.8 Etching ........................................................................................ 316 7.9 Pellicles ....................................................................................... 316 7.10 Mask-Defect Inspection and Repair ............................................ 324 Problems ............................................................................................... 328 References............................................................................................. 329 Chapter 8
Confronting the Diffraction Limit .................................. 345
8.1 Off-Axis Illumination ................................................................. 345 8.2 Optical Proximity Effects............................................................ 354 8.3 The Mask-Error Enhancement Factor (MEEF)........................... 365 8.4 Phase-Shifting Masks .................................................................. 368 8.5 Putting It All Together ................................................................ 379 Problems ............................................................................................... 383 References............................................................................................. 383 Chapter 9
Metrology ......................................................................... 391
Linewidth Measurement ............................................................. 391 9.1.1 Linewidth measurement using scanning electron microscopes.................................................................... 391 9.1.2 Scatterometry ................................................................. 402 9.1.3 Electrical linewidth measurement .................................. 405 9.2 Measurement of Overlay ............................................................. 408 Problems ............................................................................................... 412 References............................................................................................. 413 Chapter 10 Immersion Lithography and the Limits of Optical Lithography ..................................................................... 419 10.1 Immersion Lithography............................................................... 419 10.2 The Diffraction Limit .................................................................. 426 10.3 Improvements in Optics .............................................................. 428 10.4 Maximum Numerical Aperture ................................................... 430 10.5 The Shortest Wavelength ............................................................ 433 10.6 Improved Photoresists ................................................................. 435 10.7 Flatter Wafers.............................................................................. 436 10.8 How Low Can k1 Go? ................................................................. 437 10.9 How Far Can Optical Lithography Be Extended? ...................... 438 10.10 Multiple Patterning ..................................................................... 441 10.11 Interferometric Lithography........................................................ 447 Problems ............................................................................................... 449 References............................................................................................. 449
Chapter 11 Lithography Costs .......................................................... 455 11.1 Cost-of-Ownership ...................................................................... 455 11.1.1 Capital costs ................................................................... 457 11.1.2 Consumables .................................................................. 466 11.1.3 Mask costs ...................................................................... 467 11.1.4 Rework ........................................................................... 468 11.1.5 Metrology ....................................................................... 469 11.1.6 Maintenance costs .......................................................... 469 11.1.7 Labor costs ..................................................................... 470 11.1.8 Facilities costs ................................................................ 470 11.2 Mix-and-Match Strategies........................................................... 470 Problems ............................................................................................... 473 References ............................................................................................. 473 Chapter 12 Extreme Ultraviolet Lithography ................................... 475 12.1 Background and Multilayer Reflectors ....................................... 475 12.2 EUV Lithography System Overview .......................................... 480 12.3 EUV Masks ................................................................................. 485 12.4 Sources and Illuminators ............................................................. 492 12.5 EUV Optics ................................................................................. 497 12.6 EUV Resists ................................................................................ 502 Problems ............................................................................................... 507 References ............................................................................................. 509 Chapter 13 Alternative Lithography Techniques ............................ 523 13.1 Proximity X-ray Lithography...................................................... 523 13.2 Electron-Beam Direct-Write Lithography .................................. 529 13.2.1 Single-beam direct-write systems .................................. 532 13.2.2 Multiple-electron-beam direct-write systems ................ 534 13.2.3 Cell-projection lithography ............................................ 538 13.2.4 Scattering-mask electron-projection lithography ........... 538 13.3 Ion-Projection Lithography ......................................................... 541 13.4 Imprint Lithography .................................................................... 542 13.5 Directed Self-Assembly .............................................................. 544 Problems ............................................................................................... 548 References ............................................................................................. 549 Appendix A Coherence ....................................................................... 557 Problems ............................................................................................... 560 References ............................................................................................. 561 Index ..................................................................................................... 563
Preface to the Fourth Edition This new edition of Principles of Lithography is long overdue, since there have been many advances in lithographic technology since the 3rd edition was published in 2010. Since the publication of that earlier edition, EUV lithography has progressed from research to the threshold of high-volume manufacturing. There are now additional insights into the concepts regarding line-edge roughness that were described in previous editions. Mask-making is evolving with the introduction of multi-beam mask writers. As in previous editions, I have tried to emphasize the fundamental principles of lithographic technology, without delving too deeply into particular advanced topics except where such subjects are commonly used by practicing lithographers. There are many people who supported this new edition. First, I would like to thank the publications staff at SPIE for their patience and support. I would also like to thank the following people who provided figures for this edition: Dr. Michael Lercel of ASML (Fig. 5.2), Dr. Winfried Kaiser of Carl Zeiss (Fig. 5.30), Dr. Alain Diebold of SUNY Polytechnic (Fig. 9.15), Dr. Lei Sun of Metalenz (Figs. 3.37 and 9.8), Dr. William Hinsberg of Columbia Hill Technical Consulting (Fig. 12.33), Dr. Erik Hosler of GLOBALFOUNDRIES (Fig. 12.19), Dr. Jim Farrell and Ms. Theresa Chavez of AMD (figure of a Ryzen microprocessor in Chapter 1), Ms. Cherry Tang of JSR (Fig. 3.11), Mr. Rob Crowell of TEL (Fig. 3.13), Dr. Uzodinma Okoroanyanwu of the University of Massachusetts (Fig. 3.17), Dr. Hans Loeschner of IMS (Fig. 7.17), Mr. Tom Newman of AMAT (Fig. 7.18), and Dr. Ivan Pollentier of IMEC (Fig. 3.4). Mr. Peter Buck of Mentor Graphics provided the information in Table 7.6. In addition, I would like to thank the following people for permission to use figures from their publications: Dr. Juan DiPablo of the University of Chicago (Fig. 4.24), Dr. Xuemei Chen of KLA (Fig. 9.23), Prof. Glenn Fredrickson of the University of California at Santa Barbara (Fig. 13.20), Dr. Sergey Babin of aBeam Technologies (Fig. 9.9), Dr. Yulu Chen of KLA (RuSi reflectance), Dr. John Biafore of KLA (Fig. 12.24), Dr. Patrick Naulleau of Lawrence Berkeley National Laboratory (Fig. 3.49), Dr. Lieve van Look of imec (Fig. 12.13), and Mr. Matthias Ruhm of GLOBALFOUNDRIES (Fig. 6.12), and Dr. Sudharshanan Raghunathan of ASML (Fig. 12.31). Also to be thanked are several people who shared information that was incorporated into the book: Mr. Ernesto Abruna of ZYGO for references on interferometers; Dr. Martin Tschinkl of AMTC for information on mask fabrication; Dr. Obert Wood on background information on EUV lithography; Dr. Feixiang Luo for information on implant resists; Dr. Anindarupa Chunder of ix
Preface to the Fourth Edition
Applied Materials on information regarding molecular sizes; Dr. Elmar Platzgummer of IMS Nanofabrication for information on electron beam write tools; Dr. Shuo Zhao of Hermes Microvision for information on EUV lithography targets for specific process layers; Dr. Gian Lorusso of imec for information on SEM measurements of LER; Dr. Jing Jiang of Applied Materials for feedback on Chapter 3; Dr. Richard Farrell of Tokyo Electron for explanations regarding DSA and material for Fig. 13.19; and Dr. Ryan Del Re and Mr. Sung Yong Bae of GLOBALFOUNDRIES for information on resist filtering. Finally, I would like to thank my wonderful wife, Laurie Lauchlan, for her continuing support. Harry J. Levinson March 2019
Preface to the Third Edition The need to update Principles of Lithography only five years after the release of the second edition is evidence of the quickly changing and exciting nature of lithography as applied to the production of integrated circuits and other microand nanoscale devices. Since the 2nd edition was written, immersion lithography has moved from development into volume manufacturing, double patterning methods have been developed to maintain scaling using optical lithography, extreme ultraviolet (EUV) lithography has started to move from the laboratory to development pilot lines, and there has been a significant increase in skills in many other aspects of lithography. I hope that the readers of this new edition are satisfied with my efforts to explain the salient points of the newly developed technology. For students, I have added more homework problems. As a practical matter, not every contribution to lithography described in a publication could be referenced, but I do hope that I have properly recognized the work of others, while providing the reader with a tractable and useful list of references. I would like to thank the many people who contributed to this latest edition of Principles of Lithography, providing figures, papers, and explanations. Specific figures were provided by Lars Liebmann (Fig. 10.18), David Kyser of Applied Materials (Fig. 7.11), Simi George of Lawrence Berkeley Laboratories (Fig. 12.18), David Brandt of Cymer (Fig. 12.17), Hiroko Takeuchi of Nuflare (Fig. 7.6), Norihiro Yamamoto of Spansion (Figs. 7.26 and 7.27), Bruno La Fontaine of Cymer (Figs. 12.1 and 12.2), Stefan Wurm of GLOBALFOUNDRIES (Fig. 12.6), Wolfgang Holzapfel of Heidenhain (Fig. 5.36), Andreas Erdmann from the Fraunhofer Institute (Fig. 5.45), Brigette Wehrmann and Leah Rickman of Suss Microtec (Fig. 5.48), Kafai Lai of IBM (Fig. 8.34), and Paul Nealey from the University of Wisconsin (Fig. 13.20). Robert L. Brainard of the State University of New York (SUNY), Albany, provided useful information on resists for next-generation lithography. Conversations with Andrew Hazelton of Nikon regarding linewidth control and double patterning were also very useful. Christian Buergel and Fritz Gans of the AMTC supplied information on mask making and inspection. Anna Tchikoulaeva and Paul Ackmann of GLOBALFOUNDRIES provided constructive suggestions to improve the chapter on masks and reticles. Joe Daggett from Sumika provided useful information on adhesion promotion. Assistance with EUV transmission calculations from Erik Gulliksen of Lawrence Berkeley Laboratories was most appreciated. Discussions with Uzodinma Okoroanyanwu of GLOBALFOUNDRIES were helpful for understanding xi
Preface to the Third Edition
pinhole formation in ultrathin resists. Yuansheng Ma, also from GLOBALFOUNDRIES, helped significantly with the section on resist line-edge roughness. Vito Dai of GLOBALFOUNDRIES supplied expert advice on data handling for direct-write lithography. Copies of useful references were provided by Banqui Wu of Applied Materials, John Burnett of NIST, and Bert Jan Kampherbeek of MAPPER. Christian Wagner of ASML helped to clarify some subtle issues regarding EUV lithography. Eli Dagan explained the status of maskmaking tools at Applied Materials. Gavin Rider generously provided information on electrostatic damage to masks. Winfried Kaiser of Carl Zeiss helped to clarify issues relating to high-performance optics. Timothy Groves of SUNY, Albany, provided useful explanations and information on aspects of electron-beam lithography. Fabian Pease, Edward Sebesta, and John Burnett pointed out specific errors in prior editions, which I hope have now been corrected. I continue to appreciate those people who provided figures and information for the earlier editions. I would like to thank Jerry Sanders, founder of Advanced Micro Devices, whose commitment to excellence enabled many of the ideas in this book to be discovered, learned, and applied by individual engineers in service to the customer. Finally, I would like to thank my wife, Laurie, for her continuing, saintly patience and support. Harry J. Levinson August 2010
Preface to the Second Edition This book was written to address several needs, and the revisions for the second edition were made with those original objectives in mind. First, and foremost, this book is intended to serve as an introduction to the science of microlithography for people who are unfamiliar with the subject. Most papers written for journals or conference proceedings assume that the reader is familiar with pre-existing knowledge. The same can be said for compilations of chapters written by experts who are providing their colleagues and peers with useful summaries of the current state of the art and of the existing literature. Such papers and books, while quite useful to experienced lithographers, are not intended to address the needs of students, who first need to understand the foundations on which the latest advances rest. It is the intention of this book to fill that need. For the experienced lithographer, there are many excellent books written on specialized topics, such as photoresist and resolution enhancement techniques, and I have referenced many of those fine works. However, I have often felt that several topics have not been well addressed in the past; most notably those subjects directly related to the tools we use to manufacture integrated circuits. Consequently, this book goes into a few subjects in depth. These include such topics as overlay, the stages of exposure tools, and light sources. Finally, this text contains numerous references. These are resources for students who want to investigate particular topics in more detail, and they provide the experienced lithography with lists of references by topic. A wise leader once told me that one of the most challenging tasks is to transform complexity to simplicity; in other words, to make apparent the forest obscured by all of the trees. I hope that I have succeeded adequately on the subjects covered in this book. Of course, simplicity should never be confused with easiness or completeness. To assist the student in recognizing these distinctions, more problems have been added to the end of each chapter. It is expected that the reader of this book will have a foundation in basic physics and chemistry. No topics will require knowledge of mathematics beyond elementary calculus. Lithography is a field in which advances proceed at a swift pace, and many new topics have been included in this second edition, commensurate with the learning that has taken place during the past few years, and several subjects are discussed in more detail. Optical proximity corrections and next-generation lithography are examples where the landscape looks quite different than it did just a few years ago. Other topics, such as immersion lithography, were ideas that xiii
Preface to the Second Edition
few took seriously just a few years ago, yet today are considered quite mainstream. It has been my good fortune to work with a number of outstanding lithographers. In addition to the people acknowledged in the preface to the first edition, I would like to thank several people who contributed to this update. These include Tim Brunner of IBM, Wolfgang Henke of Infineon, Margaret Conkling of Nikon Precision, Nigel Farrar, Vladmir Fleurov, Palash Das and Charles Hindes of Cymer, Andreas Erdmann of Fraunhofer-Institut für Integrierte Schaltungen, Doug Resnick and John Algair of Motorola, Wilhelm Maurer of Mentor Graphics, Christian Wagner and Robert Socha of ASML, Paul Graeupner of Carl Zeiss, Johannes Nieder of Leica, John Ricardi and Harry Rieger of JMAR, Ray Morgan of Canon, USA, Walter Gibson of XOS, and Sandy Burgan of DNS. Merry Schnell and Sharon Streams of the publications staff of SPIE have been very helpful and supportive. I apologize if I have failed to mention anyone who has helped me with this update. It has also been a privilege and joy to work on a more frequent basis with some exceptionally outstanding lithographers in my own department, as well as other lithography departments, at AMD. In particular, this includes manufacturing organizations, where the principles discussed in this book have been put skillfully applied and expertly enhanced to produce high performance non-volatile memory and the world’s most powerful Windows-compatible microprocessors. From AMD, I would like to thank Bruno La Fontaine, Jongwook Kye, Ivan Lalovic, Adam Pawloski, Uzodinma Okoroanyanwu, Rolf Seltmann, Wolfram Grundke, and Rick Edwards for useful and informative discussions on lithography. I would like to thank my wife, Dr. Laurie Lauchlan, and my daughters, Sam and Sarah, who continued to exhibit amazing patience while I worked on the second edition of this book. On September 11, 2001, the world witnessed the destructive power of the irrational mind. I hope that this book will be a small reminder of the tremendous capacity of the rational human mind to improve the world around us. Harry J. Levinson January 2005
Preface to the First Edition This book has been written to address several needs. First, it is intended to serve as an introduction to the science of microlithography for someone who is unfamiliar with the subject. It is expected that the reader has a foundation in basic physics and chemistry. No topic requires knowledge of mathematics beyond elementary calculus. The book covers a number of advanced subjects as well, and it can be used by experienced lithographers who wish to gain a better understanding of topics that are not in their own areas of expertise. Numerous references are made to literature in optical lithography, providing a guide for both novice and experienced lithographers who want to learn about particular subjects in detail. A number of discussions––such as thin-resist modeling, metrics for imaging, thin-film optics, and the modeling of focus effects––first appeared in Advanced Micro Design internal reports. Eventually, some parts of these reports were published elsewhere. Their tutorial nature is not coincidental, as they were analyses that I used to develop my own understanding of lithography. It is often found that complex situations are best comprehended through simple models that describe most of the relevant physics, with the remaining effects considered as perturbations. This is the approach I used in learning lithography myself, and it is the method used in this book. Students of the class on lithography science that I periodically teach will recognize many of the figures and equations. A number of these are also used in the first chapter in the SPIE Handbook on Microlithography, Micromachining, and Microfabrication, Volume I: Microlithography, which I coauthored with Bill Arnold of ASM Lithography. Additional topics have been added or expanded significantly, especially those concerning light sources, photomasks, and next-generation lithography. The chapter on overlay is an expanded version of a similar chapter found in my earlier text, Lithography Process Control (SPIE Press, 1999). The chapter on photoresists takes a different approach from that found in most books on lithography. Here, resists are approached from the perspective of the practicing lithographer, rather than the resist chemist. Some resist chemistry is discussed because this knowledge is essential for using resists properly, but the emphasis is on operational considerations. A number of acknowledgments are in order. First, there are several people at AMD to be thanked. Jongwook Kye provided the data for Figs. 8.8, 10.4, and 10.5. Figure 12.8 shows two micrographs, generated by Janice Gray, of an EUV mask fabricated at AMD. Dr. Uzodinma Okoroanyanwu has provided the author with guidance through the world of resist chemistry. Figure 3.26 was contributed by Marina Plat. xv
Preface to the First Edition
It has been my good fortune to have had the opportunity to interact with many of the world’s experts in lithography, and their works are referenced throughout this book. Quite a number of the ideas presented in this book first appeared in papers that I coauthored with Bill Arnold, who is now Executive Scientist at ASM Lithography. I have also had a long association with Dr. Moshe Preil of KLA-Tencor, and we have written several papers together. Lithographers at semiconductor companies are integrators. We combine optics, precision machines, photochemicals, and photomasks into working processes. While chip makers often get the glory, the lens makers, resist chemists, and tool makers are the unsung heroes of the microelectronics revolution. It has been my good fortune to be able to interact with many of the world’s experts in optics, equipment, and lithographic materials. A number of people have provided assistance in the writing of this book. Several people at Carl Zeiss (Dr. Winfried Kaiser, Dr. Christian Wagner, Dr. Bernd Geh, and Dr. Reiner Gerreis) have explained elements of lens optics and metrology to me. Bernd Geh donated the data of Fig. 4.6, Winfried Kaiser provided Fig. 5.15, and Figs. 5.21 and 5.25 were provided by Dr. W. Ulrich. Figure 5.2 was obtained from Roy Wetzel of ASM Lithography. Dr. Don Sweeney of Lawrence Livermore Laboratory provided Fig. 5.19, and offered generally useful information on EUV technology, as did Dr. Dan Bajuk, Dr. Saša Bajt, and Dr. David Attwood. Figure 5.9 was obtained from Bob Willard of Lambda Physik. Figure 2.25 was provided by Wes Brykailo of the Shipley Company. The data in Figs. 3.9, 3.10, and 3.11 were contributed by Eddie Lee, Emir Gurer, Murthy Krishna, and John Lewellen of Silicon Valley Group. Figure 3.14 was a donation from Will Conley of Motorola, and Dr. Sergey Babin of Etec provided Fig. 7.14. Dr. Rainer Kaesmaier of Infineon and Dr. Hans Löschner of IMS Vienna were particularly generous in providing information on ion-projection lithography, including Figs. 12.13 and 12.14. Kurt Heidinger of the Cyantek Corporation supplied information on wet chromium etchants. I want to thank Phil Seidel for providing the data of Fig. 11.1. Dr. Chuck Gwyn of Intel contributed Fig 12.10. Dr. David Joy helped to improve my understanding of SEM metrology. Bill Moffat of Yield Engineering tutored me as a young engineer and more recently on adhesion promotion. The references would be far less complete without the excellent services provided by AMD’s librarians, John Owen, Wendy Grimes, and Sharon Shaw. I apologize to anyone who has helped me put together this book and has not been acknowledged. Finally, I would like to thank my wife, Dr. Laurie Lauchlan, who provided me with a true appreciation of the importance of metrology, and for her apparently infinite patience while I wrote this book. This book is dedicated to Laurie, and our daughters, Samantha and Sarah. Harry J. Levinson April 2001
Principles of Lithography Fourth Edition
Chapter 1 OVERVIEW OF LITHOGRAPHY The patterns of integrated circuits are created on wafers by lithography. The steps of this critical manufacturing process are listed in Table 1.1. Each step will be discussed at length in later chapters of this book, but a brief description of each will be given here. Most of this book is devoted to photolithography, where optical methods are used to transfer the circuit patterns from master images— called masks or reticles—to the wafers. Photolithography is the method used for patterning nearly all integrated circuits fabricated today. Adhesion promotion: The lithography process creates the patterns of integrated circuits in films of specialized materials called resists, which are coated onto the wafers on which the circuits are made. Resists typically do not adhere properly to untreated surfaces of silicon or silicon-containing materials, such as silicon dioxide and silicon nitride. To ensure proper adhesion, the wafer surfaces are treated prior to resist coating. Resist coat: Resists typically comprise organic polymers applied from a solution. To coat the wafers with resist, a small volume of the liquid resist is first dispensed onto a wafer. The wafer is then spun about its axis at a high rate of spin, flinging off the excess resist and leaving behind, as the solvent evaporates, a thin (0.1–2.0 m, typically) film of solid resist. Table 1.1 The steps in the lithography process. The steps in italic are optional. Adhesion promotion Resist coat Softbake Alignment Exposure Post-exposure bake Development Hardbake Measurement and inspection
Softbake: After the resist coating has been applied, the density is often insufficient to support later processing. A bake is used to densify the resist film and drive off residual solvent. Alignment: Integrated circuits are fabricated by a series of patterning steps. These start with a lithography operation followed by an etch or ion implantation. Between patterning steps, there may be film depositions, planarizations, and other processes. Each new pattern must be placed on top of preceding layers, and proper overlay of the new layer to the circuit pattern already on the wafer is achieved during the alignment step by using specialized equipment. Exposure: Photoresists are materials that undergo photochemical reactions when exposed to light. There are two types of photoresists––positive and negative. Positive resists are normally insoluble in the chemicals referred to as resist developers, but are made soluble by exposure to light. Negative resists have the opposite behavior: they are soluble in developer and rendered insoluble by exposure. By exposing the resist selectively in some areas and not others, the pattern of the circuit can be created in the resist film. This selective exposure is accomplished in optical lithography by the imaging of a mask. Photomasks are sheets of glass, partially covered by an opaque material, usually chromium, that has been removed according to the pattern of the circuit. By shining light onto the mask, and then projecting the transmitted image onto the resist film, the pattern of one layer of the circuit is transferred to the resist film on the wafer. Post-exposure bake: This is an optional baking step used to drive additional chemical reactions or the diffusion of components within the resist film. The purposes of the post-exposure bake are discussed in Chapters 3 and 4. Development: This is the step by which a resist is removed, depending upon whether or not it has been exposed. Measurement and inspection: This is an optional operation where it is determined by measurement if the resist features on the wafer are sized correctly and properly overlay preceding patterns, and that they are sufficiently free from defects. These measurements may be used for the purposes of process control or dispositioning. Hardbake: This is another optional process. Because wafers with photoresist patterns nearly always go into etch or ion implantation operations immediately following the lithography step, a final bake is often used to drive out volatile organic materials and water in order to preserve the vacuum integrity of the etch and ion implantation equipment. The temperature required for this step is usually so high that it will degrade the photochemical properties of the resist. Had the high-temperature hardbake been employed prior to the development step, the resist would not have developed properly. Consequently, the hardbake is one of
Overview of Lithography
the last steps in the lithography process, though it may precede measurement and inspection. The role of the lithography process in overall integrated circuit fabrication can be appreciated by considering the sequence of deposition, lithography, and etch steps used to establish electrical contacts to the transistors that make up integrated circuits (Fig. 1.1). Electrical interconnections are made after the transistors have been fabricated and covered with insulating oxide or another suitable dielectric. The wafers are then covered with resist, and the resist is exposed in places where electrical contacts to the transistors are desired. For reasons explained later, positive resists are commonly used for making electrical contacts. The exposed resist is developed out, exposing the oxide above the points where electrical contact is desired. The wafer is then put into an environment of oxide etchant. The oxide still covered by resist is protected against the etch, while the oxide is removed where electrical contact is desired. The contact holes can then be filled with metal, thus establishing electrical contact. The primary tool used for projecting the image of the circuit from a photomask onto a resist-coated wafer is the wafer stepper. Wafer steppers exist in two configurations––step-and-repeat and step-and-scan. In a step-and-repeat system, the wafer is positioned under a lens so that a projected image of the layer to be exposed will properly overlay the patterns already on the wafer (Fig. 1.2).
Figure 1.1 The sequence of steps used to make electrical connections in a planar transistor in an integrated circuit.
Figure 1.2 Exposure of resist-coated wafers on wafer steppers.
The systems that allow the stepper to bring the wafer into proper position are discussed in Chapter 6. Once the wafer is properly positioned and brought into focus, a shutter in an illumination system is opened, allowing light to pass through the photomask. The pattern on the mask is then imaged by the lens onto the wafer. The image is reduced laterally by the amount N:1, where N is the lensreduction factor, most commonly equal to 4 in leading-edge systems today. Values of N of 1, 2, and 2.5 are found on steppers that have been designed primarily for high productivity. Large values of N are desirable to the extent that they reduce the effects of variations in linewidths and misregistration on the reticle, generally by the factor of N, as the image of the reticle is projected onto the wafer. Defects are also reduced in size to the point that they often fall below the resolution limit of the lens. The first commercially available wafer stepper, the GCA DSW4800, had N = 10. However, as chip sizes became larger, smaller values of N were required to avoid reticles that were bigger than what was practical. For many years, most steppers had lens-reduction factors of 5, but values of 4 began to appear in the early 1990s. They are found on all leading-edge systems today. For a given mask size, larger exposure fields on the wafer are possible with smaller values of N, and systems designed for high productivity (but not necessarily to produce the finest patterns) often have N < 4. With larger exposure fields, fewer fields need to be exposed in order to pattern wafers completely, which gives an opportunity for higher throughput. Because of reduction by the projection optics, only part of the wafer (an “exposure field”) is exposed at any one time on a wafer stepper. After one field is exposed, the wafer is moved on an extremely precise stage so that another part of the wafer can be exposed. This process of exposure and wafer stepping is repeated until the entire wafer is exposed. In the typical reduction stepper, the stage travels in the horizontal plane beneath a fixed, vertically mounted lens.* * The Micrascan systems on which wafers moved vertically were exceptions but are no longer being manufactured. These exposure tools were originally made by Perkin-Elmer. The Perkin– Elmer exposure tool business was purchased by SVG, Inc., which in turn was acquired by ASML.
Overview of Lithography
Figure 1.3 Step-and-repeat and step-and-scan configurations.
In a step-and-repeat system, the entire area of the reticle to be exposed is illuminated when the shutter is opened. In a step-and-scan system, only part of the reticle, and therefore only part of the exposure field on the wafer, is exposed when the shutter is opened (Fig. 1.3). The area exposed on step-and-scan systems at any instant is usually a narrow rectangular region, referred to as the slit. The entire field is exposed by scanning the reticle and wafer synchronously. The reticle stage must be scanned at a speed of N times faster than the wafer, where N is the lens-reduction factor. (The motivations for scanning are discussed in Chapter 5.) This method of fabrication is extremely efficient, since many circuit features are patterned in parallel. For example, a NAND flash memory will have two contacts per bit in the memory arrays. With 34-nm design rules, four 32-Gb NAND flash memory chips are exposed simultaneously on a step-and-scan system when the mask is illuminated. Consequently, over 256 billion contacts are imaged in a single exposure, which occurs in about 0.1 sec. If one thinks of this in terms of a transfer of design information to the wafer, where each contact is considered to be a single piece of information, this is a remarkable rate of information transfer: over 2.5 trillion bits of information are transferred per second. Moreover, this rate of transfer continues to increase as lithography processes become able to print smaller features. This increasing rate of transfer, driven by the ability to print features of decreasing size, is the key factor in the reduction of the cost of microelectronics. Each step of the lithographic process is discussed in this book. Pattern formation is of central importance because the great functionality of modern microelectronics has been enabled by the ability to pack large numbers of individual transistors in a unit area of silicon. The principles of optics relevant to imaging small features are covered in Chapter 2, while photoresists are discussed
in Chapter 3. Methods of predicting lithographic performance are presented in Chapter 4. The primary tool used in lithography—the wafer stepper—is described in Chapter 5, and this leads into overlay, the topic of Chapter 6. Mask technology is the subject of Chapter 7. Advanced methods of optical lithography are reviewed in Chapter 8. The problem of measuring the small features created by the lithography process is addressed in Chapter 9. The limitations imposed by the laws of physics on optical methods are discussed in Chapter 10. Lithography costs, which can be as significant as technical issues, are covered in Chapter 11. Finally, possible next-generation lithography options that might succeed optical lithography are reviewed in Chapters 12 and 13.
For a mask that is 152 152 mm, and assuming that a 10-mm border at the edges of the plate is required to hold the mask, show that the largest field that can be patterned on the wafer is 13.2 13.2 mm if the lens-reduction factor is 10. What is the largest field if the factor is 5? 4?
The area of the AMD Ryzen microprocessor is 213 mm2 (22 9.7 mm):
Can such a die be printed in a single exposure with an exposure tool with 10× lens reduction? 4× lens reduction? Why do you think that large lensreduction factors are not used, even though their use would reduce the criticality of reticle quality? 1.3
What are the nine principal steps in the lithographic process? Which steps are optional?
In the lithographic process, what are the materials called in which patterns are formed on the wafers?
Chapter 2 OPTICAL PATTERN FORMATION 2.1 The Problem of Imaging The basic problem of imaging is shown in Fig. 2.1. Light from an illumination source passes through a photomask (often referred to as a reticle), which defines the patterns. The simple photomask illustrated here consists of two types of complementary areas—one type that is opaque, while the other is transparent. In this example, the transparent (or “clear”) area is a long space of uniform width, and the optical and resist profiles shown in Fig. 2.1 are cross sections for this geometry. Some of the light that passes through the mask continues through a lens, which projects an image of the mask pattern onto a wafer. The wafer is coated with a photosensitive film, a photoresist that undergoes a chemical reaction upon exposure to light. After exposure, the wafer is baked and developed, leaving regions covered by photoresist and complementary regions that are not covered. The patterning objective of microlithography is to produce well-defined resist features, sized within specifications. This is a challenge because of the shape of the light-intensity distribution produced at the wafer plane by a lens of finite resolution. This distribution lacks a clearly defined edge (Fig. 2.1). From the light-intensity distribution alone, it is not possible to know where the edges of the feature are. If the light-intensity distribution had the shape shown in Fig. 2.2, there would be no such problem, because a clear delineation would exist between areas of the resist exposed to light and areas unexposed to light. The light distribution shown in Fig. 2.1 was not drawn arbitrarily or artistically. Because light is a form of electromagnetic radiation, it is possible to use equations that describe the propagation of electromagnetic waves to calculate optical image formation,1 and the light-intensity distribution shown in Fig. 2.1 was generated accordingly. The physics of image formation will be discussed in more detail in this and later chapters. Lithographic processes are easier to control the closer the actual optical images resemble the ideal ones. If the light profile at the wafer plane is represented by the distribution shown in Fig. 2.2, the edges of the feature could be clearly identified by looking at the light-intensity distribution. The photoresist on the wafer would be cleanly separated into exposed and unexposed areas. In the situations that actually occur, the photoresist receives continuously varying doses of light in the regions corresponding to features on the mask. Proper pattern definition on the wafer requires that small differences in exposure doses at the edges of pattern features be distinguished through the resist processing. Edge control will be better for light-intensity distributions that closely resemble the ideal case illustrated in Fig. 2.2. 7
Figure 2.1 An illustration of the imaging process. Light passes through a reticle (photomask). The resulting pattern is imaged onto a photoresist-covered wafer by a lens. The finite resolution of the lens results in a light-intensity distribution that does not have clearly defined edges. The particular light-intensity distribution shown in this figure was calculated using PROLITH 1.5, for a 0.25-μm space on a 0.65-μm pitch (i.e., for a grating pattern of 0.25-μm spaces and 0.4-μm lines), where the numerical aperture (NA) of the aberration-free lens is 0.5, imaging at a wavelength of 248 nm, and with 0.5 partial coherence. The parameter “numerical aperture” will be explained later in this chapter, and partial coherence is discussed in Appendix A. Actinic refers to light that drives chemical reactions in the photoresist.
Figure 2.2 An ideal light-intensity distribution.
Optical Pattern Formation
Figure 2.3 Light-intensity profiles for 150-nm isolated spaces (nominal). One image was generated for an aberration-free 0.7-NA lens, with a partial coherence of 0.6, at a wavelength of 248 nm (KrF), and the other image was generated for a 193-nm (ArF) unaberrated lens, with NA = 0.75 and a partial coherence of 0.6. These images, all in the plane of best focus, were calculated using the simulation program Solid-C.2 The ArF lens has higher resolution than the KrF lens.
Figure 2.4 Calculated light-intensity distributions for isolated spaces of varying sizes, using parameters for an aberration-free 0.7-NA lens, with a partial coherence of 0.6, at a wavelength of 248 nm. All of the features are normalized to a width of 1.0. All images are in the plane of best focus.
Light-intensity profiles produced by two sets of optics, one of “higher resolution” than the other, are shown in Fig. 2.3. (The parameters that affect image sharpness and resolution will be discussed later in this chapter.) The image produced by the higher-resolution lens is closer to the ideal image than the one produced by the lens with lower resolution. For a given feature size, it is possible to have better pattern definition with higher-resolution optics. However, because of the highly competitive nature of the microelectronics industry, lithographers need to operate their processes at the limits of the best available optics. With a given set of optics, the light-intensity distributions are degraded further, relative to the ideal case, with smaller features (Fig. 2.4). As features become smaller, the
edge slopes of the light-intensity profiles become more sloped, and the peak intensity decreases. The challenge for lithographers is to produce the smallest possible features on the wafers, with shape and size well controlled, for a given generation of optics.
2.2 Aerial Images The origin of the image-intensity profile of Fig. 2.1 is the physical phenomenon of diffraction, a subject that was studied extensively in the nineteenth century and is well understood.1 Diffraction effects are inherent to the wave nature of light. The resolution of optical tools is fundamentally limited by the physical phenomenon of diffraction, and as device geometries shrink, the lithography engineer must ultimately contend with this barrier imposed by the laws of physics. This is illustrated in Fig. 2.4, where aerial images are shown for features of varying sizes. As the feature size shrinks, the edge acuity of the light-intensity distribution is degraded. If even smaller features are considered, at some point one must say that features are no longer resolved, but it is clear from Fig. 2.4 that there is a gradual transition from “resolved” to “unresolved.” A definition of resolution is not obvious because of this lack of a clear delineation between “resolved” and “unresolved.” Simple diffraction analyses lead to the most frequently cited quantitative definition of resolution, the Rayleigh criterion, which will be introduced shortly. While sufficiently instructive to justify discussion, the Rayleigh criterion does not provide a measure directly applicable to the situation encountered in photolithography, and one should use it with care. Discussion of the Rayleigh criterion in this book emphasizes its assumptions and therefore its applicability. The subjects of diffraction and image formation are quite involved and, at best, can only be introduced here. The mathematical formalism is particularly complex, and the interested reader is referred to the references cited at the end of this chapter. The phenomenon of diffraction will be introduced through two examples—the diffraction grating and the circular aperture. The origin of the resolution limits of optical systems can be appreciated by considering the system shown in Fig. 2.5. A reticle with a diffraction grating with a periodicity 2d (equal lines and spaces) is illuminated by a source of coherent light of wavelength . (For readers unfamiliar with coherence, a short introduction is provided in Appendix A.) For an angle of incidence of θi, the grating diffracts the light into various beams whose directions are given by1
sin sin i
m , m 0, 1, 2,... . 2d
Here we are assuming that the index of refraction of air, which surrounds the mask and lens, is 1.
Optical Pattern Formation
Figure 2.5 A situation with coherent light and a diffraction grating on the reticle. A ray of light is diffracted into beams that propagate in distinct directions given by Eq. (2.1).
Figure 2.6 The finite size of lenses limits the angles at which diffracted beams are collected.
Consider a lens with a collection angle of θ0 (Fig. 2.6) used to image the grating. Due to Eq. (2.1), the lens collects only a finite number of diffraction beams. Coherent light illuminating a grating diffracts into beams that correspond to the object’s Fourier components, and a diffraction-limited lens will recombine those beams that pass through the entrance pupil of the lens. If the lens collects all of the diffracted beams, then the grating will be fully reconstructed in the image. However, since the lens collects only a finite number of beams the image is only a partial reconstruction of the original grating pattern. As light from increasingly larger angles is collected, the image consists of more terms in the
Fourier-series expansion of the light-intensity distribution of the grating (see Fig. 2.7). For on-axis illumination (θi = 0), 2
m mx 1 2 1 . I ( x) I 0 sin cos d 2 m 1 m 2 m
If the lens captures only a single beam, then there is no pattern in the image, since a single plane wave has no spatial variation in its intensity: 2
Intensity of a single plane wave = A0 eik x A0 .
At least two interfering plane waves are needed to generate spatial variation. To retain more than the first (constant) term in the expansion of I(x), 0 must be large enough to capture diffracted beams for m 1 . For on-axis illumination, Eq. (2.1) then leads to the following expression for a minimally resolved feature: d 0.5
. sin 0
The resolution is found to be directly proportional to the wavelength of the light and inversely proportional to sinθ0. Resolution is limited because only a finite number of diffracted beams pass through the entrance pupil of the lens.
Figure 2.7 Partial sums of Eq. (2.2), with I0 = 1. The image more closely approximates a rectangular grating when more terms are added.
Optical Pattern Formation
The phenomenon of diffraction can be appreciated further by considering the situation in which uniform illumination is normally incident on a masking screen where there is a circular hole (Fig. 2.8). Such a situation arises, for example, if the light is produced by a point source located far from the masking screen. The light that passes through the hole illuminates another screen. In the absence of diffraction, the incident light would simply pass through the aperture and produce a circular illuminated spot on the second screen. Because of diffraction, in addition to the normally incident rays of light, some light propagates at divergent angles. For certain configurations, the light-intensity distributions resulting from diffraction can be obtained analytically, and the circular aperture, illustrated in Fig. 2.8, is one of these. The solution for the light intensity is plotted in Fig. 2.9. Rather than a circular beam propagating in a single direction, the light is distributed over angles that are functions of the wavelength of the light and the diameter of the circular aperture. For light of wavelength the light-intensity distribution at radius r on the imaging screen is given by1 2
J ( x) I ( x) I 0 2 1 , x
where x = dr/z, d is the diameter of the aperture, z is the distance between the two screens, and J1 is the 1st-order Bessel function. I0 is the intensity at the peak of the distribution. It should be noted that shorter wavelengths and larger apertures lead to less angular divergence. The light-intensity distribution given by Eq. (2.5) is called the Airy pattern, after G. B. Airy, who first derived it.3 Because of the diffraction that occurs at the entrance pupil or edges of a lens producing divergent beams, the images of point objects are focused Airy patterns.
Figure 2.8 A circular aperture illuminated by a point source of light.
Figure 2.9 The light-intensity distribution from a point source (of unit intensity) projected through a circular aperture in an opaque screen. The dimensions x and y are given in units of d/z, where d is the diameter of the aperture, and z is the distance between the two screens.
Rayleigh used the above property of diffraction to establish a criterion for the resolving power of telescopes, using the following argument.4 Suppose there are two point sources of light (stars) separated by a small angle. Being independent sources, the light rays from different stars do not interfere, i.e., they are mutually incoherent. Accordingly, the total light intensity is the sum of the individual intensities. The two stars are said to be minimally resolved when the maximum of the Airy pattern from one star falls on the first zero of the Airy pattern from the other star. This occurs when x 0.61 . 2
The resulting total light intensity due to the two stars with an angular separation given by x = dr/z = 0.61 × 2 is plotted in Fig. 2.10, where two peaks can be clearly distinguished. It was thus learned that the resolving capability of optical instruments is limited simply because of the finite entrance pupil. For focusing optics, the minimum resolved distance δ between the peak of the Airy distribution and its first zero can be related using criteria that must be satisfied for focusing optics, resulting in 0.61
, n sin
Optical Pattern Formation
Figure 2.10 Light-intensity distribution of two light sources projected through a circular aperture.
where n is the index of refraction of the medium surrounding the bottom of the lens (n 1 for air), is the wavelength of the light, and 2 is the angle illustrated in Fig. 2.11. The quantity nsin is called the numerical aperture (NA) of the lens. Proper lens design is required for the numerical aperture, and hence the resolution, to be uniform across the exposure field. The minimum separation given by Eq. (2.7) is referred to as the Rayleigh resolution. Examples of wavelengths and numerical apertures typically used in semiconductor processing are given in Table 2.1 along with the accompanying Rayleigh resolution. As can be seen from this table, a high resolution (small feature size) can be achieved with a large NA or a short wavelength. When focus is taken into consideration, these two paths to resolution are not equivalent, as is discussed shortly.
Figure 2.11 The angle defined by the aperture in a lens determines its numerical aperture.
Table 2.1 Typical parameters for stepper optics. Year of first use refers to the first year of use in high-volume manufacturing (HVM). The sources for 13.5-nmwavelength light are discussed in Chapter 12.
Wavelength Numerical (nm) aperture 436 0.30 365 0.45
Rayleigh resolution 0.89 µm 0.49 µm
Year of first use 1982 1990
Light source Hg arc lamp (g line) Hg arc lamp (i line)
Hg arc lamp (i line) Hg arc lamp or KrF excimer laser KrF excimer laser
KrF excimer laser
ArF excimer laser
ArF excimer laser
ArF excimer laser
It is worth restating that the Rayleigh criterion for resolution is obtained by considering the imaging of point sources of light, which is not the situation encountered by photolithographers. The geometries on photomasks that must be imaged onto the front surface of wafers are extended in size, generally approximating the size and shape of a circuit element. The resolution problem is shown in Fig. 2.4. As the features become smaller, the optical profile becomes flatter, and it becomes increasingly difficult to locate the “edge” of a feature. As is discussed later, linewidth control is directly related to the slope of the optical intensity distribution. Although it was derived for a situation different from those encountered by lithographers, the Rayleigh criterion for resolution is nevertheless useful as a scaling equation. For example, if one increases the numerical aperture by 20%, the optical resolution is also expected to change by ~20%, even if the exact value of the minimally printed linewidth is not given by Eq. (2.7). For the microelectronics industry, the relevant issue is not the “resolution” of point sources, but rather how small features that exist in real integrated circuits (IC) can be printed. In the context of microelectronics processing, the minimum printable feature size is also dependent upon the properties of the photoresist, while the Rayleigh criterion was derived solely on the basis of optical considerations. As resists improve, the minimum feature size that can be printed becomes smaller for fixed optics. To take advantage of the scaling property of the Rayleigh criterion, and the dependence on resist processes, Eq. (2.7) is often rewritten as
Optical Pattern Formation
smallest feature k1
where NA is the numerical aperture, and the prefactor of 0.61, associated with point sources, is replaced by k1 (usually referred to as the “k factor” for a given process). For a given resist system, Eq. (2.8) provides scaling, and the prefactor changes if a different photoresist process is used. The imaging analysis of a grating structure contains a curious feature associated with coherent illumination. For a particular set of optics, grating dimensions are resolved to a certain point and then not resolved at all for smaller features, at the point when the multiple beams no longer enter the lens. This behavior of optics, where its performance falls off rapidly as the rated resolution limits of the lenses are approached, is familiar to most photolithographers. The extremely sharp cutoff in resolving power of the grating example in this book is an artifact of the complete coherence of the light and single direction of the illumination. This cutoff led to a situation in which terms of the expansion Eq. (2.2) were retained with their complete magnitudes or not retained at all. For partially coherent and incoherent light, the coefficients of the cosines in the image-series expansion decrease more gradually as the diffraction limits are approached, and as the illumination includes light incident from multiple angles. Consider again the mask pattern consisting of a grating of a periodicity of 2d. Near the resolution limit, the image consists of only a constant plus a single cosine term that has the same periodicity as the mask pattern, regardless of the configuration of the optics. After passing through the optical system, the lightintensity profile appears as shown in Fig. 2.12. The minimum light intensity Imin is greater than zero, and the peak light intensity Imax is less than the illumination intensity. The optical contrast or modulation is defined as 5, 6 C
I max I min . I max I min
Figure 2.12 Light intensity as a function of position, for a grating pattern on the reticle.
The optical contrasts of grating structures for different types of illumination, as a function of spatial frequency, are plotted in Fig. 2.13. The spatial frequencies are related to feature size by the relationship
1 . 2d
High spatial frequencies correspond to small features. In the case of diffractionlimited optics (that is, optics where the imaging performance is limited only by the phenomenon of diffraction and not by lens quality), the transfer characteristics can be plotted in terms of normalized spatial frequencies o, where o = /NA. As shown in Fig. 2.13, there is a sharp cutoff for image contrast with completely coherent illumination, with no image contrast resulting for features smaller than 0.5 NA/. For incoherent and partially coherent light, the image contrast degrades, and there is no similar distinction between features that can and cannot be imaged with good contrast. The amount by which sinusoidally varying intensities of incoherent light diminish as they pass through an optical system is called the modulation transfer function (MTF)7 and has been used not only within the context of photolithography, but also to characterize the resolving capabilities of optics. For optics with circular apertures, the functional form of the MTF is known and, for aberration-free optics, is given by
Figure 2.13 Contrast [defined in Eq. (2.9)] of the image of a grating, produced by an in-focus diffraction-limited lens. The normalized spatial frequency is given by λ2dNA, where 2d is the period (or pitch) of the grating, NA is the numerical aperture of the lens, and λ is the wavelength of the light. The coherence factor σ is defined in Appendix A. For incoherent light, the contrast equals the MTF.
Optical Pattern Formation
2 ( cos sin ) ,
for 2 NA / , where is the spatial frequency, and cos 1 . 2NA
The circular aperture MTF = 0 for > 2 NA / . This MTF function is plotted in Fig. 2.13. For incoherent illumination, the image of a diffraction grating is given by7 1 2 1m mx m m cos I ( x) I 0 MTF . sin 2 d 2d 2 m 1 m
The illumination used in microlithography is neither completely coherent nor incoherent, and the curves shown in Fig. 2.13 for coherent or incoherent light do not accurately characterize the transfer properties of mask features onto wafers. The contrast of partially coherent light, more typical of the illumination encountered in the context of optical lithography, is also shown in Fig. 2.13. When operating in a region where the optical contrast curve is relatively flat, the imaging variations among features of different sizes are small. As the resolution limit of the lens is approached, the imaging capabilities of the lens fall off quickly. The greater the coherence of the light, the greater the optical contrast is up to the resolution limit, but there is a sharp cutoff for small features. Patterns in photoresist can be generated for optical contrasts less than 1.0, but significantly greater than zero; the exact number depends upon the resist system. The partial coherence of exposure tools is chosen to provide the optical contrast necessary for patterning minimum-sized features in single layers of photoresist. Metrics for optical-image quality other than contrast are used more extensively today, and these are discussed later in this chapter. The preceding discussion has described several general properties of optical systems. First and foremost, the resolution of an optical system is limited by the physical phenomenon of diffraction. This limit may not be reached in actual optical systems because of lens aberrations, which are discussed in Chapter 4. The sharpness of the resolution “edge” of a lens is dependent upon the degree of coherence of the illumination, and for exposure systems that have been used in the past, the falloff in optical contrast becomes steep as the resolution limit is approached, but it is not perfectly sharp. Creating resist images within manufacturing tolerances, and on a repeatable basis, from poorly defined optical profiles is the challenge confronting microlithographers. Fortunately, there is more to lithographic pattern formation than optics. Photoresist is a second key ingredient for patterning. One can think
of a lithographic-exposure system as essentially a camera in which the photoresist plays the role of the film. Following the development process, a pattern is formed in the photoresist. The quality of the final resist patterns is determined by the resolving power of the optics, the focusing accuracy, the contrast of the resist process, and an assortment of other variables that cause the final image to be a less-than-perfect reproduction of the features on the mask. Just as common film for personal cameras produces pictures of varying quality depending upon the film’s photospeed, contrast, and graininess, as well as the focus setting of the camera, the final images produced photolithographically are affected by the resist processes and the optics used. An understanding of the independent factors that contribute to pattern formation and their interactions is essential for the photolithographer. For example, consider the situation in which a production process has started to produce poorly defined patterns. Is the problem due to the resist process or the exposure system? An understanding of the various contributions to the final image enables the lithography engineer to resolve the problem expeditiously. Process-development engineers must also have a solid understanding of the fundamentals of lithography. For a new process, advanced optics provide high resolution at the expense of capital, while sophisticated resist processes might extend the capabilities of any optics, but with a possible increase in process complexity (and other issues discussed later). By appreciating the roles that the resist and optics play in pattern formation, the photolithography engineer can design the most cost-effective and capable manufacturing line. An overview of the lithographic process is presented in this chapter whereby the separate contributions from the optics and the resist process can be seen. Each subject is then discussed in more detail in subsequent sections. Two characteristics of the final resist pattern are of primary interest—the size and the shape. Processes capable of producing the narrowest possible linewidths are highly desired because they enable smaller chips to be produced, allowing large numbers of devices to be produced on each wafer. Thus, there is a tight connection between lithographic capability and profits. Short gates are also needed for fast electronics. The requirements of the resist shape are usually imposed by the post-lithographic processing. Consider, for example, the situation in which the photoresist is to serve as a mask for ion implantation. If the edges of the resist are nearly vertical, normally incident implantation is clearly delineated by the resist edge, resulting in a sharp doping profile. On the other hand, if the resist has considerable slope, high-energy ions penetrate the partial thickness of the resist at the edges of the pattern, and the resulting doping profile is graded. The relevance of the resist-edge slope and its effect on the doping profile depends upon the overall process requirements. Another common example in which the slope of the resist is important occurs when the resist is to be used as a mask for plasma or reactive ion etching, and the etching process erodes the photoresist. The slope of the photoresist can be transferred to the etched layer, which may or may not be desirable. There is no lithographic consideration that purely determines the optimum process. However, once the requirements of the
Optical Pattern Formation
final resist pattern are determined from considerations of the post-lithographic processing, the masking process can be specified. Typically, the most preferred resist profiles are ones that are nearly vertical. Since these are generally the most difficult to produce, as well as the most desired, our discussion is oriented toward such profiles. Regardless of the specific size and shape requirements of the resist patterns, which may vary from one technology to another, all lithographic processes must be consistent and reproducible, relative to manufacturing specifications, in order to be appropriate for use in production. The parameters that affect process uniformity and consistency must be understood, as well as those that limit the ultimate performance of a lithographic tool or process. Identification of those parameters is a subject of a significant portion of this chapter. A typical resist profile is shown in Fig. 2.14. The shape of the cross section is often idealized as a trapezoid. Three dimensions are of greatest interest: the width of the resist line at the resistsubstrate interface, the slope of the sidewall, and the maximum thickness of the resist film after development. Of course, actual resist profiles often depart significantly from the idealized trapezoid. The Semiconductor Equipment and Materials International (SEMI) standard that defines linewidth8 accounts for such departures, and linewidth is defined to be a function of the height from the resistsubstrate interface (Fig. 2.15). Throughout the next section, if the word “linewidth” is used with no further clarification, it is understood to be the dimension L = y2 – y1 measured at the resistsubstrate interface. This definition has been chosen for three reasons. First, the width at the base of the resist line is of greatest relevance to the result after the post-lithographic processing. For example, in a highly selective etch where there is little resist erosion, all other dimensions of the resist line have negligible influence on the resultant etch. Moreover, in the presence of a sloped resist profile, the definition adopted here for linewidth is unambiguous. Finally, the value of the linewidth is decoupled from the slope of the resist line.
Figure 2.14 (a) Cross section of Sumitomo PAR101 resist, printed on an ASML 5500/900 193-nm step-and-scan system, which had a 0.75 NA. (b) Idealized trapezoid cross section.
Figure 2.15 The SEMI standard definition for linewidth. Linewidths are given by the quantities L = y2 – y1 defined at the distances x0 along the resist line and at height z0.
At this point, the astute reader has noted that the term “resolution” has not been given a rigorous definition. Since the ability of lithography to resolve small features is a driving force in the microelectronics industry, a definition of this key quantity might appear to be in order. The use of theoretically based measures, such as the Rayleigh criterion, are useful for gaining insight into the lithography process and estimating capability, but they are not completely adequate because they fail to account for imperfect lens design and manufacture. They are also insufficient for other reasons. For example, a lithography process might be unable to reproduce a pattern coded for 50 nm on the reticle (50 nm times the lens reduction), but adjustments to exposure in the same process might allow 50-nm features to be formed on the wafer by overexposing larger features (for example, 100 nm times the lens reduction) on the reticle. Depending on one’s perspective, the resolution of the lens could be considered either 100 nm or 50 nm. The resulting ambiguity is a consequence of an additional variable, print bias, which is the difference between the size of the feature on the mask (divided by the lens reduction) and the size of the corresponding feature patterned in resist on the wafer. Similarly, optics have different capabilities for imaging isolated lines, isolated spaces, square contacts, or isolated islands. Should resolution be considered for one type of feature or for all features, with or without print bias? The answers to these questions are user dependent, making it impossible to assign the parameter “resolution” to particular optics, or even a particular lithography process, in a way that meets all of the widely varying needs. Nevertheless, one can speak as to whether particular features are resolved, within context. For a particular circumstance, limits can be placed on linewidth, slope, resist thickness, etc. Once these limits are specified, a feature can be said to be resolved so long as it fits within the limits. However, the sizes and shapes of resist patterns that can be considered acceptable in the most important circumstances (integrated circuit manufacturing lines) depend upon the requirements of post-lithographic processing.
Optical Pattern Formation
When considering the limits of optical lithography (a topic discussed in detail in Chapter 10), the pitch is typically the most relevant parameter. The principal benefit of advanced lithographic technology is the ability to pack large numbers of connected transistors onto a small area of silicon. It is this capability that enables enormous device functionality to be available at low prices. The smallest line printable with an optical system is much smaller than the half-pitch. One may be able to print such small lines, but that capability does not directly address the challenge of packing a large number of connected transistors onto a small area. Such capability is useful for high-performance logic systems, so it is not without value; however, when describing the limits of lithographic systems, it is most useful to express them in terms of the half-pitch. For evaluating and comparing optical systems, these problems may be circumvented by choosing a particular resist process as a reference process, with pre-established requirements for linewidth variations, slope, etc. Other resist processes can be characterized as well by comparison with the reference process. Elegant definitions of resolution may be appropriate in a laboratory environment, while the masking engineer needs quantities that can be determined with the tools at hand. There are many ways to characterize the resolution capabilities of optical systems,9,10 but in the end the resolving capabilities of a lithography exposure system are usually determined by inspecting photoresist patterns. By using such a method, the contributions from the resist process influence the patterning. It is appropriate at this point to discuss the role of photoresist in pattern formation.
2.3 The Contributions of Physics and Chemistry With some basic concepts in hand, we can now start to explore the photolithographic process through some simple models.11,12 The first step in developing a model is the assignment of numerical values to the light-intensity profiles, such as those depicted in Figs. 2.1, 2.3, and 2.4. The light intensity is modulated spatially by the mask and further modified by the optics of the lithography equipment. Because we are considering only a long space of glass in the photomask in this illustrative example, the light intensity I at the plane of the wafer is a function I(x) of only one variable, where x is the distance at the wafer plane along the direction perpendicular to the space. To simplify the discussion, we also initially assume the substrate, which is coated by the resist film, to be flat and nonreflecting. Effects due to substrate topography and reflectivity are addressed later. The basic assumption for this simple model is that the thickness T(x) of photoresist remaining after development is determined by the exposure energy dose E(x) = I(x) ꞏ t, where t is the exposure time:
T ( x) TE ( E ) TE [ E ( x)] .
This is a reasonable assumption for very thin or high-contrast photoresist. For positive photoresist, greater exposure results in thinner resist films, while negative resist remains thicker with higher exposures. The current discussion is restricted to positive photoresists. A typical plot of TE(E), normalized to the initial thickness T0, is shown in Fig. 2.16 and is called the “characteristic curve” of the resist, following similarly named curves used for characterizing photographic films.13 Such a curve may be obtained by exposing large areas on a wafer with different exposure energies and then measuring the residual thicknesses in those areas after development. To be precise, the characteristic curve is not only a property of the resist but also of the entire resist process, and it depends upon the developer and process parameters such as bake temperatures. Several features of the curve should be noted. First, there is a flat region at low exposure where little resist is removed. In this part of the curve, the final thickness may not be equal to the thickness T0 of the resist film before exposure, since the developer may remove some of the resist even though it is unexposed. Typically, resist-thickness loss in unexposed or less exposed regions is 20 to 200 Å. Second, there is an exposure dose E0 above which the photoresist film is completely removed. This dose is referred to as the dose to clear or E-zero. Finally, the curve is linear (with a logarithmic scale for the abscissa) in the region around E0:
TE E T0
E ln 0 , E
for E < E0. The slope is called the “contrast” of the resist process and is defined by Eq. (2.15). Typical values for are shown in Table 2.2.
Figure 2.16 A typical characteristic curve for photoresist, showing the thickness remaining after development as a function of exposure dose. Resist thickness is plotted on a linear scale, while the exposure dose is plotted on a logarithmic scale to produce a curve that is approximately linear in the vicinity of E0.
Optical Pattern Formation
Table 2.2 Resist contrast for selected photoresists.15–18 As noted, contrast is a property of the resist process, not just the resist material. The contrasts listed in this table are for typical optimized processes.
Resist Exposure wavelength (nm) Contrast () Reference AZ 1470 436 5.8 15 Shipley 511 365 6.9 16 Apex E 248 4.7 17 TOK IP3000 365 6.8 18
Figure 2.17 A space in (positive) resist is created by exposure and development. The resist thickness T(x) is a function of x.
The dependence of the shape of the final resist pattern on the resist process can be seen in the following analysis. The slope of the resist sidewall is simply dT tan , dx
where the derivative is evaluated at the point x0 where the resist profile and the substrate intersect (Fig. 2.17). Note also that E0 = E(x0).
Equation (2.16) can be expressed as14 dT dTE dE . dx dE dx
Equation (2.18) neatly divides the factors that determine the resist profile. The first factor, dTE/dE, is characteristic of the photoresist and development process, independent of the exposure tool, while the second factor, dE/dx, is completely determined by the optics of the exposure system. One obtains dTE/dE by differentiating a curve such as the one shown in Fig. 2.16 but on a linear scale. The function E(x) is discussed shortly. In the vicinity of x0, TE(E) is described by Eq. (2.15). This results in the following expression for the slope of the resist profile: tan
1 dE ( x) dT T0 . dx E ( x) dx
Steeper resist profiles are produced with high-contrast resists (large values of ) and steep optical profiles, which have large values for the normalized derivative, (1/E)(dE/dx). Our simple model is based upon the assumption that the resist development behavior that has been measured in large exposed areas can be applied directly to situations where the light intensity is modulated over small dimensions. This is equivalent to assuming that T(x) is solely a function of E(x). Within the limits to which our assumption is valid, the dependence of the profile slope is cleanly separated into the contributions from the optics [the factor (1/E)(dE/dx)] and from the resist process (represented by ), and each can be studied independently of the other. Theoretical models of image formation in projection optics have been developed, usually starting from the Hopkins formulation for partially coherent imaging.19 The Hopkins theory is based on scalar-wave diffraction theory from physical optics. Imaging models provide the engineer with the ability to calculate E(x) for various configurations of optics. Let us consider the optics term E(x) and its normalized derivative, (1/E)(dE/dx). E(x) was calculated for a “perfect” lens using a commercially available simulation program, Solid-C,2 and the results are shown in Figs. 2.4 and 2.18. All profiles are shown in normalized dimensions so that for each feature size the mask edges occur at 0.5. The normalized derivative is shown only around the region of interest, close to the edge of the mask feature. As one can see, for fixed optics the “sharpness” of the opticalintensity profile degrades and the value of 1/E(dE/dx) at the edge of the mask feature is clearly reduced as the feature size is decreased. Lens aberrations or defocus would also reduce the magnitude of 1/E(dE/dx), while higherresolution optics would increase its value. Since Eq. (2.19) is nonlinear, substantial degradation of the optical contribution to the profile slope can be tolerated if the contrast of the resist process is large enough.
Optical Pattern Formation
Figure 2.18 Absolute values of calculated normalized derivatives (image log slope) (1/E)(dE/dx) of the intensity distributions shown in Fig. 2.4, near the position in the image that corresponds to the mask edge at x = 0.5. The center of the feature occurs at x = 0. Overexposure corresponds to values of x > 0.5.
It should be noted that 1 dE 1 dI , E dx I dx
where E is the exposure dose, and I is the corresponding light intensity, since
E I t ,
where t is the exposure time. All of the expressions involving the normalized derivative of the image can be written equivalently in terms of exposure dose or light intensity. One can express the normalized derivative of the intensity or dose as 1 dE d ln E , E dx dx
if one is willing to disregard technical rigor. (A logarithm of a parameter with dimension, such as length, mass, etc., is not a well-defined quantity.) Because of Eq. (2.22), the normalized derivative of the dose (or intensity) is often referred to as the image log slope (ILS). Another advantage of a high-contrast resist process becomes apparent when one is trying to print over a surface that is not flat. Since resist, when spun on the wafer, tends to planarize,20–22 masking over an underlying feature is equivalent to patterning photoresist of varying thickness. This can be seen in Fig. 2.19. If the
thickness of the photoresist is changed from T0 to T0 + T, with all other aspects of the lithographic process remaining equal, then the edge of the photoresist line moves from x0 to x0 + x, and the minimum exposure energy required to clear the resist to the substrate changes from E0 to E0 + E. After exposing the thicker resist with energy E0, the amount of resist remaining is T. By drawing a new characteristic curve for thicker photoresist, as seen in Fig. 2.20, the slope in the linear region is given as a result of
T T T , 0 E ln 1 E0
T E T0 E0
for small variations. (It is assumed here that the resist is on a nonreflecting substrate. The more complex situation in which the substrate is reflecting is discussed in Chapter 4.)
Figure 2.19 Resist (dark material at the top of the figure) spun over topography has a relatively planar top surface.
Optical Pattern Formation
Figure 2.20 Characteristic curve for thicker photoresist. The ordinate is the thickness of the resist remaining after development, normalized to the resist thickness T0 + T0, while the abscissa is the natural logarithm of the dose normalized to E0 + E.
The shift in the edge of the photoresist line that occurs due to the change in the thickness T of the photoresist is given by x
E , dE / dx
where the derivative is evaluated at the point x0. From Eq. (2.24), this becomes T x T
1 dE E0 dx
T 1 ILS . T
The change to linewidth as a function of resist thickness is kept small by having resists of high contrast, and optics with large image log slopes. Again, there is a separation between the optical term, which reappears in the form of the normalized derivative (or image log slope) (1/E)(dE/dx), and the photoresist, whose contribution is expressed through the quantity . It is also interesting to explore exposure latitude, i.e., the sensitivity of the linewidth to the exposure dose, in terms of our simple model. If the exposure dose is changed fractionally from E to (1 + f ) E, then the edge of the resist line is moved from x0 to x0 + x (Fig. 2.21).
Figure 2.21 With a change in dose, there is a shift in position where the light intensity equals a threshold value.
The edge of the resist line is still determined by Eq. (2.17): (1 + f ) E(x0 + x) = E0 = E(x0) .
dE x fE x0 , dx
E . E
We then obtain an expression for the change in linewidth (ΔL = 2|Δx|): 1
E ( x) 1 d L 2 E ( x) , E ( x) E ( x) dx L 2
E ( x) 1 ILS , E ( x)
Optical Pattern Formation
where all expressions are evaluated for x at the line edge. Our expression for exposure latitude [Eq. (2.31)] contains only factors involving the exposure optics and is independent of the photoresist process and its characteristics. Since it is observed empirically that exposure latitude can be modulated to some degree through the resist process, it is clear that the model presented here is not exactly valid, but it is good to the 1st order and best within the limits of thin- or highcontrast photoresist. In several expressions—those for resist slope [Eq. (2.19)], variation of linewidth with changing resist thickness [Eq. (2.27)], and exposure latitude [Eq. (2.32)]—it can be seen that the lithography process is more controllable with a large image log slope (see Table 2.3). For this reason, the image log slope was introduced as a metric of image quality11 and continues to be widely used.23 Additional critical parameters related to the image log slope are discussed in later chapters. Higher-resolution optics can affect the printing of large objects, as well as enable the printing of smaller features. Consider the light-intensity profiles for a 150-nm feature, shown in Fig. 2.3. The higher-resolution optics provide sharper images, which results in larger image log slopes (Fig. 2.22), at least for the best focus. The normalized derivative at the edge of the space increases from 15 m–1 for the 0.7-NA lens with 248-nm-wavelength illumination to 27.m–1 for the 0.75-NA lens at 193-nm-wavelength illumination, an increase of nearly 2. According to the results of the previous section, this translates into direct increases in exposure latitude and linewidth control. Such behavior has led to the proposal that resolution be defined by exposure latitude. From Fig. 2.22, it can be seen that the image log slope is not determined uniquely by the parameters of the optics, such as exposure wavelength, numerical aperture, degree of partial coherence, aberrations, etc. The value of the normalized derivative 1/E(dE/dx), which affects the exposure latitude, resist wall profile, and linewidth control over steps, depends not only on the resolution of the optics but also on the print bias as well, that is, the point at which the derivative is evaluated. The value of 1/E(dE/dx) at the mask edge is different from that at other positions. The normalized derivative is evaluated at the position x0, which is the edge of the resist line, and may not correspond to the edge of the feature on the mask. The resist patterns may have dimensions Table 2.3 Several key lithography parameters in relation to the image log slope. Parameter
Relation to the image log slope (ILS)
tan T0 ILS
L 2E ( x) / E ( x) ILS
Linewidth change with resist thickness
x (T / T ) ILS
Figure 2.22 Absolute values of normalized derivatives of the light-intensity distributions shown in Fig. 2.3, given in units of μm–1.
different from the ones on the mask. If the spaces in (positive) resist are printed larger than the ones on the mask, then they are termed “overexposed,” and if they are printed smaller, they are called “underexposed.” Resist patterns having the same dimensions as on the mask are termed “nominal.” Resulting from overexposure or underexposure, the quantities that depend upon the normalized derivative, such as exposure latitude, are functions of the print bias. This is seen quite clearly in Fig. 2.22, where the best exposure latitude occurs for overexposure. As is explained in the next section, this result is true only so long as focus is well maintained and the situation in which the optics are significantly defocused is more complex. Higher-resolution optics improve the image log slope and hence many parameters, such as resist profiles and exposure latitude. Unfortunately, higherresolution optics are never acquired simply to make the photolithographer’s job easier. When higher-resolution optics become available, the challenge is simply shifted to smaller features, where the normalized derivative remains small. From the preceding, an expression for the exposure latitude is given by E L L 1 d E ( x) . E L 2 E ( x ) dx
In terms of the image log slope, one can rewrite this equation as E L L ILS . E 2L
Optical Pattern Formation
The quantity in parentheses is referred to as the normalized log slope. This is important to recognize, since image log slopes need to increase as feature sizes decrease in order to maintain constant exposure latitude. When discussing exposure latitude particularly among different feature sizes, the normalized log slope is the appropriate parameter. As a consequence, a related metric, with an additional normalization related to the nominal linewidth L is often used, namely, the normalized image log slope (NILS): 1 dE NILS L . E dx
The above results show how the optics and resist processes play separate and somewhat independent roles in image formation. Of course, the performance of the lithographic process is also determined by practical issues not captured in theoretical models, such as resist adhesion, and many of these problems are discussed in later chapters. In the analysis presented in this section, the role that photoresist plays is related to its development rate as a function of exposure. The study of optics and its role in photolithography reduces to the analysis of E(x) and the parameters that determine its values. The focusing of the image has a significant effect on E(x), as is seen in the next section.
2.4 Focus In earlier discussions, the light-intensity distributions were considered only in the planes of best focus. In optical systems, defocus occurs when the separation between the imaging plane and the lens is different from the optimum. From common experience, one knows that defocus reduces the clarity of optical images. The image produced by a common overhead projector may be slightly out of focus, but the presentation may remain readable. If the defocus becomes too great, the image is unintelligible. In lithography, the depth-of-focus concept is the range of lenswafer distances over which linewidths are maintained within specifications, and resist profiles are adequate. The problem of defocus is particularly acute in optical lithography, where the depth-of-focus is becoming so small that it is a concern as to whether optical wafer steppers are capable of maintaining the image in focus. The problem of defocus can be appreciated by considering the imaging of a point source of light. In purely geometrical optics, where it is assumed that light travels in straight lines, a point object will be imaged by ideal optics to a point located in the focal plane (Fig. 2.23). However, in other planes, the point source of light is broadened into a circle. When imaging, there is generally an amount of broadening that is considered acceptable. Conceptually, the range of values of z over which this broadening remains acceptable is the depth-of-focus. At a given distance z from the focal plane, it can be seen that the broadening will be greater
for larger values of . It might therefore be expected that lenses will have decreasing depths-of-focus with increasing numerical aperture. (Compare Figs. 2.11 and 2.23.) In the discussion of the imaging of a grating structure, it was noted that gratings with smaller lines and spaces created diffracted beams at larger angles [Fig. 2.5 and Eq. (2.1)]. From this consideration, one can also expect that objects with smaller feature sizes will have smaller depths-of-focus. This shows that there is a tradeoff between resolution and depth-of-focus. Lenses with larger numerical apertures may be used to resolve small features, but the resulting images will have smaller depths-of-focus than the corresponding images of larger features imaged by lower-NA lenses. The diffraction of a point source of light by a circular aperture discussed earlier (Fig. 2.9) has been extended to the situation in which a lens is used to image the point source of light. The resulting calculated light-intensity profiles in different focal planes are shown in Fig. 2.24. With defocus, the peak intensity diminishes and more light is diffracted away from the center spot. Using the criteria that the peak intensity should not decrease by more than 20%, the following expression results for a depth-of-focus (DOF):1 DOF 0.5
Figure 2.23 In geometrical optics, a point source imaged by an ideal lens is focused to a point in the focal plane. Away from the plane of best focus, the image is a circle of radius r.
Optical Pattern Formation
Figure 2.24 Light-intensity profile of a point source of light imaged by a circular diffraction-limited lens at different planes of focus. The horizontal axis is given in units of πdNA/λ, where d is the diameter of the lens aperture. One Rayleigh unit of defocus is 0.5λ/NA2.
which is valid for small to moderate values of NA and imaging in air. Over this range of focus, the peak intensity of a point object focused by a lens remains within 20% of the peak value for best focus, where NA is the numerical aperture of the lens, and is the wavelength of the light. This expression is usually referred to as the Rayleigh depth-of-focus; one Rayleigh unit of defocus is 0.5/NA2. The situation for large values of NA will be discussed in Chapter 10. It is useful to use the Rayleigh criterion for estimating the depth-of-focus encountered in photolithography. Typical parameters for 180-nm lithography are = 248 nm and NA = 0.6, which result in a Rayleigh depth-of-focus of 0.34 m. That is, the distance between the lens and the wafer needs to be controlled to this very small amount. The small depth-of-focus in optical lithography, and the associated process-control problem, is the reason that focus is given a great deal of attention by lithographers (including the author of this book). Just as the Rayleigh criterion for resolution was generalized, Eq. (2.36) is often written in the form DOF k2
Equation (2.37) is expressed as a total range, instead of distances from a midpoint, because the symmetry of the aerial image is broken by the photoresist or optical aberrations in actual application, and the depth-of-focus is often
asymmetric about the plane of best focus in high-resolution optical lithography. This asymmetry is discussed later in this section. The Rayleigh expressions for resolution and focus both depend upon only two lens parameters—the wavelength and the numerical aperture—and a pair of constants, k1 and k2. One can then relate resolution R and depth-of-focus: DOF (constant)
Within the framework of this analysis, one can see that the depth-of-focus diminishes as one attempts to print smaller features (smaller R). From the Rayleigh criterion for resolution, there are two options for improving resolution: decreasing the wavelength or increasing the numerical aperture. Doing either of these also decreases the depth-of-focus, at least according to Rayleigh. However, improving resolution by decreasing the wavelength has less effect on the depthof-focus than by increasing the numerical aperture. This is the primary reason that leading-edge optical lithography has involved the use of decreasing wavelengths in the pursuit of smaller features. The Rayleigh criteria might lead one to a false conclusion that the depth-offocus diminishes whenever one attempts to improve the resolution of the optics. From the following argument, one can appreciate that this is not true. Suppose one has a lens that has a resolution of 1.0 m, i.e., it does not image features smaller than this. One could therefore say that such a lens has zero depth-offocus for submicron features. A higher-resolution lens capable of submicron resolution therefore has greater depth-of-focus for smaller features. This line of reasoning leads to the observation that there is an optimum numerical aperture that is a function of feature size.12,24–28 At one time, improper interpretations of the Rayleigh criteria led to the conclusion that optical lithography would not be able to break the 1.0-mresolution barrier. However, photolithography has produced, in volume production, fully functional, large-scale devices with 140-nm pitches, i.e., minimum features ~70 nm. Furthermore, it continues to be the dominant method of patterning feature design rules to 45 nm and even smaller (using techniques that will be described in Chapter 8). Just as the Rayleigh criterion was insufficient for defining the resolution of optics, in the context of photolithography there are additional considerations to be examined for understanding focus and depth-of-focus. The depth-of-focus of the lens depends on the feature size and type being imaged. As the NA is increased, the limiting resolution becomes finer, but the depth-of-focus for larger features becomes smaller. The optimum NA and partial coherence values depend on the size and type of geometry being imaged, as well as the type of illumination and degree of coherence. The degree of partial coherence is defined in Appendix A. For example, the optimum NA to image a contact hole is higher than what is needed for a grating of equal lines and spaces
Optical Pattern Formation
of the same size on the reticle, and greater depth-of-focus (for lines and spaces) is achieved with higher values of . The dependence of imaging on feature size, shape, and surroundings has led to wafer steppers with variable parameters, such as numerical aperture and partial coherence. Because resolution is not useful without adequate depth-of-focus, the concept of practical resolution29,30—the resolution achieved with some specified depth-of-focus—is helpful for defining the optimum NA, , and other process parameters. For the situation encountered in lithography, the effects of defocus can be readily observed. Shown in Fig. 2.25 are cross sections of lines and spaces of resist as focus is varied. Clearly, the sidewall slope increases for large defocus. As shown in Fig. 2.25, linewidths also vary with focus, and the sensitivity of linewidths to defocus is a function of the exposure dose and print bias.31
Figure 2.25 Resist profiles for imaging 105-nm lines (320-nm pitch) at best focus and various amounts of defocus. The KrF resist was UV110, patterned on a SiON antireflection coating, using annular illumination ( = 0.75 outer, 0.50 inner) on an ASML 5500/300 (NA = 0.60, = 248 nm), which is described in Chapter 8.
As defined earlier, the depth-of-focus is the distance by which the separation between the lens and the wafer can be changed while maintaining linewidths within specifications, with adequate resist profiles, and sufficient resist thickness. The numerical value for the depth-of-focus can be compared to the capability of the exposure tools for controlling the distance between the lens and the wafer. As long as the exposure tools and the methodology used to control focus errors can maintain this distance tighter than the depth-of-focus, the process is capable. There are a number of detractors to the depth-of-focus relative to the diffraction limit. Even with an aberration-free lens, the depth-of-focus found in practice may be different than expected from consideration of the aerial image alone because the finite thickness of the resist influences the depth-of-focus. This is a consequence of refraction at the air-resist interface and the need to maintain a good aerial image throughout the entire thickness of the resist film, not just in a single plane. Typical resist thicknesses (0.1–0.2 m) are on the order of the Rayleigh depths-of-focus of contemporary high-resolution lenses. Consequently, one might expect that variations in the light-intensity distributions in the direction parallel to the optical axis should be relevant to how resist profiles are generated. In this case, the thin-resist model discussed earlier does not provide accurate predictions. This can be appreciated from simple geometrical optics. Consider a point source of light focused by a lens, as shown in Fig. 2.26. In the limit of geometrical optics, where diffraction effects are ignored, the light is focused by the lens to a point in the plane of best focus. In any plane (perpendicular to the optical axis) other than the plane of best focus, the image is a circle. The distance along the optical axis in which such circles have an acceptably small diameter is the depth-of-focus. If diameters of the focused image vary appreciably throughout the thickness of the resist film, then a more sophisticated model for the optical image than has thus far been discussed needs to be considered.
Figure 2.26 Refraction of light at the airresist interface, its effect on the position of focus, and the spreading of the image due to defocus.
Optical Pattern Formation
To understand the effects of thick resist on imaging, let us refer to Fig. 2.26. Suppose that a maximum image radius r is acceptable. For an optical image in air, the depth-of-focus would then be
2r , tan 0
where 0 is the largest angle for incident rays of light and is related to the numerical aperture by
sin 0 NA .
When a thick layer of resist is placed in the vicinity of best focus, refraction becomes a factor. In Fig. 2.26, two focused light rays converge to the point F1 instead of the focal point F0 because of refraction at the airresist interface. The angle 1 between the normal and the refracted ray is related to θ0 by Snell’s law:
sin 0 n
where n is the index of refraction of the photoresist. The depth into the photoresist through which these light rays can travel before they diverge a lateral distance greater than 2r is increased from Eq. (2.39) to DOF
2r . tan 1
This leads to an effective increase in the depth-of-focus, over the aerial image, by a factor of tan 0 tan 1
For small angles, this is approximately equal to the photoresist’s index of refraction n. That is, the reduction in the depth-of-focus due to resist thickness T is T/n. For photoresist, typical values for n are in the neighborhood of 1.7. The refraction at the resistair interface also breaks the symmetry of an unaberrated image about the plane of best focus, and is an effect seen in detailed lithography simulations.32
For well-defined and controlled patterns, good imaging needs to be maintained throughout the thickness of the resist film that may vary over topography. A rigorous capturing of the effect of device topography on the depth-of-focus is tricky because there are linewidth variations due to thin-film optical effects (to be discussed in Chapter 4) that reduce the overall process window. Even on nonreflective substrates, there are changes in linewidths because of variations in resist thickness, and these would occur even for aerial images with infinitely large depths-of-focus. Consequently, the reduction in the depth-of-focus due to topography can be considered to be T/n, where T is the largest-value resist thickness across the topography. It is important that linewidths are good simultaneously throughout the entire exposure field. The concept of usable depth-of-focus follows from the understanding that, in the practical world of integrated circuit manufacturing, imaging needs to be good for all points within a field to ensure complete circuit functionality. This philosophy, where all points within a field need to be good simultaneously, was first discussed in detail in the context of overlay,33 but the basic concepts are applicable to all lithographic parameters, including focus. The depth-of-focus of a given feature in a particular orientation can be determined for a given set of optics and resist process. However, this does not represent the depth-of-focus that can be used for making integrated circuits because integrated devices typically have geometries of many different orientations distributed over the area of the chip. It has become accepted practice to distinguish between the usable depth-of-focus (UDOF) and the individual depth-of-focus (IDOF).34 The IDOF is the depth-of-focus at any one point in the image field, for one particular orientation. The UDOF is the amount by which the separation between the wafer and the lens can be changed and still keep linewidths and resist profiles adequate throughout the entire exposure field. UDOF is the common range of all IDOFs over the printable area and all orientations. This is generally much smaller than the depth-of-focus at any individual point in the field (IDOF). There are many factors that cause the UDOF to be less than the IDOF. Astigmatism is one such factor, and it refers to situations in which lines of different orientation have different planes of best focus. An example of the consequence of astigmatism is shown in Fig. 2.27. In this figure, the vertical spaces are well resolved, but the horizontal spaces are so defocused that the resist pattern is bridged. This is an extreme example, patterned on an early 5 stepper. For modern exposure systems, the distances between focal planes for objects of different orientation are less than 50 nm and typically lead only to differences in linewidth, rather than extreme consequences, such as bridging. For a cylindrically symmetric lens, such as those typically found in lithography exposure tools, one would expect astigmatism to occur between geometries parallel to a radius vector (sagittal) and perpendicular to the radius vector (tangential). This is certainly true for astigmatism that results from the design. However, astigmatism can occur between geometries of any orientation in any part of the field because of lens manufacturing imperfections. For example, the
Optical Pattern Formation
Figure 2.27 An example of astigmatism. This is a top-down micrograph of rectangles of resist separated by trenches. The vertical spaces in the resist are well resolved, but the horizontal lines are so defocused that they are bridged.
many lens elements that comprise a stepper lens may not all be centered perfectly on a common optical axis, thereby breaking the symmetry in the center of the lens field and potentially causing astigmatism where none would be possible for a truly cylindrically symmetric system. Another focus-related aberration is field curvature. As a result of this aberration, the surface of best focus is a section of the surface of a sphere rather than a plane, and focus is not constant throughout an exposure field. As seen in Fig. 2.28, good focus can be maintained at some points within the exposure field, but most of the field suffers from some defocus because of field curvature. For both astigmatism and field curvature, the rays of light from a given point on the reticle are all focused to a single point in the image, but the collection of such points are not always in a single plane. Astigmatism and field curvature reduce the usable depth-of-focus, which is the amount that the distance between the lens and wafer can be varied and still maintain good imaging, as illustrated in Fig. 2.29.
Figure 2.28 Field curvature.
Figure 2.29 Usable depth-of-focus is smaller than the individual depth-of-focus because of astigmatism and field curvature.
Typical specified depths-of-focus for various wafer steppers are given in Table 2.4. The amount of defocus that results in significant changes in either slope or linewidth should be noted: it ranges between 1.5 and 0.4 m, and has been decreasing over time. This should be compared to the amount of focus variation that can be induced within a process (Table 2.5). All parameters in Table 2.5, except for stepper focus control and the metrology figure,35 refer to variations across an exposure field. In the preceding discussion, it was shown that the relevant value for circuit topography is the actual height of circuit features divided by the index of refraction of the photoresist. Table 2.4 Typical depths-of-focus for various wafer steppers. Resolution and depth-of-focus are given for approximately comparable conditions across technologies and exposure platforms. As will be shown in Chapter 8, techniques have been developed over time to improve resolution and depth-of-focus significantly. Usable Stepper Resolution (µm) depth-of-focus (µm) GCA 4800 1.25 1.50 Nikon 1.00 1.50 Canon 0.80 1.20 ASML 5000/50 0.50 1.00 Micrascan 2+ 0.30 0.80 ASML 5500/300 0.25 0.70 Canon ES2 0.15 0.40 ASML 5500/950 0.15 0.40
NA Wavelength Year 0.28 g-line 1980 0.35 g-line 1984 0.43 g-line 1987 0.48 i-line 1990 0.50 KrF 1995 0.57 KrF 1996 0.68 KrF 1999 0.63 ArF 2000
Optical Pattern Formation
Table 2.5 Parameters in a typical focus budget. Parameter Typical values (range, in nm) Chuck nonflatness 30 Lens field curvature, astigmatism 20 Wafer nonflatness 40 Stepper focus control 20 Circuit topography 30 Metrology for determining focus 20 Total (sum) 160 Total (rss) 68
As lenses improved, with significant reductions in field curvature, astigmatism, and other aberrations, the UDOF began to approximate the Rayleigh DOF. More recently, new imaging methods, referred to as resolutionenhancement techniques (RETs), have been adopted. These new techniques have made it possible to achieve larger depths-of-focus than the Rayleigh DOF. After the year 2000, the UDOF specified by exposure-tool suppliers usually takes into account that some of these techniques are used. Resolution-enhancement techniques will be discussed in more detail in Chapter 8. The actual focal range over which imaging must be good is typically somewhere between the sum total of the parameters in Table 2.5 and the rootsum-of-squares (rss) total, since some of the components tend to act randomly (wafer nonflatness, stepper focus control), while others are systematic components (circuit topography). As one can see, the values for these parameters are comparable to the depths-of-focus for high-resolution optics. One common misconception is that optical lithography is limited by diffraction when the depth-of-focus becomes less than the thickness of photoresist. Such a misunderstanding results from not rigorously distinguishing between the DOF of the aerial image and the operationally measured DOF, which is performed using resist of finite thickness. The operationally measured DOF automatically captures the effects of resist thickness. Consequently, it is quite possible to speak of having a process with a 0.5-μm-thick resist layer and a 0.4-m DOF. The 0.4 m refers to the range over which the 0.5-μm layer of resist can be moved while maintaining resist linewidths and profiles within specifications. Changes in linewidth as a function of focus and dose are shown in Fig. 2.30. At a given dose, the linewidths change with defocus. It should be noted that the amount of linewidth change as a consequence of defocus depends upon the exposure dose. A dose at which there are minimal linewidth changes when the image is defocused is referred to as the isofocal dose. The thin-resist models used in the preceding section to illustrate the concepts of resolution can be extended to considerations of focus. The light-intensity distribution can be calculated for planes other than the plane of best focus;
Figure 2.30 Linewidth as a function of focus for dense lines.36 The process conditions were: softbake and post-exposure bake at 110C for 60 sec, and puddle development for 52 sec in AZ 300 MIF developer at 22C exposed on a Nikon 0.54-NA i-line wafer stepper. Curves such as these are referred to as Bossung curves.31
examples are shown in Fig. 2.31. As can be seen, the optical-intensity profiles degrade with defocus. However, there are positions where the light intensity changes little, or not at all, with defocus. Processes that are set up to have the edges of developed resist features correspond to these positions generally have small changes in linewidth. These positions are known as the conjugate or isofocal points,37 and they are usually close to the nominal line edges, i.e., the resist linewidths have approximately the same dimensions as those on the reticle (adjusted for the reduction ratio of the projection optics). They correspond to the isofocal dose. Earlier, it was seen that the normalized derivative of the optical-intensity profile at best focus was increased by having a substantial exposure bias. As derived, parameters such as exposure latitude, linewidth control over topography, and resist sidewall slope are improved with a large normalized derivative. In the absence of defocus, one would conclude that a large print bias would lead to an optimized process. In the presence of defocus, the normalized derivative behaves differently, as shown in Fig. 2.32. At best focus, the image log slope increases for a significant amount of print bias. The magnitude of the image log slope diminishes at all print biases for defocus, but the degradation is greater away from the conjugate point. For sufficiently large defocus, the image log slope actually decreases with print bias. Thus, one is led to a significantly different conclusion concerning the advantage of large print bias when defocus is a significant concern. It was shown earlier in this chapter that the process window is increased with a large image log slope. However, it is often advantageous to compromise the image log slope if there is a limited depth-of-focus.
Optical Pattern Formation
Figure 2.31 Calculated light-intensity distributions at different focus settings for a 300-nm space exposed at λ = 248 nm, NA = 0.5, and σ = 0.6. Defocus is measured in units of microns (μm).
Figure 2.32 Absolute values of the normalized derivative (image log slope) of the light-intensity profiles shown in Fig. 2.31. The normalized derivative is in units of μm–1, and defocus is measured in μm.
The thin-resist model of the preceding section can be extended to include defocus, in which case the light-intensity profile becomes a function of two variables: E ( x ) E ( x , ) ,
where x refers to the distance parallel to the wafer plane and perpendicular to the (long) resist lines and spaces, and ξ is the amount of defocus. The condition that determines the position of the edge of the photoresist is E0 E x0 , E x0 x, .
Expanding the right side of Eq. (2.45) in a Taylor series about the plane of best focus, the linewidth change due to defocus is obtained: 1
1 2 E 1 E 2 1 2 . 2 E0 E0 x
Derivatives in x are evaluated at the point x0, and derivatives in are evaluated at best focus, = 0. In the Taylor expansion, the linear terms in are zero because E 0
in the plane of best focus, and higher-order terms in x were dropped from Eq. (2.46). The symmetry of the aerial image about the plane of best focus is expressed by Eq. (2.47). In the presence of photoresist, or certain optical aberrations, this symmetry is broken. This is not particularly problematic where the thin-resist model is a valid approximation, but it can be relevant for situations involving high numerical apertures and thick (relative to the Rayleigh DOF) photoresist. In prior discussions, process latitude was improved when the image log slope (the normalized derivative), 1 E , E0 x
is increased. For example, as seen in Fig. 2.18, the image log slope at best focus may be maximized for overexposed spaces, an operating point often distant from the isofocal point. Consequently, there may be large variations in linewidths because of defocus, offsetting any benefits of a large image log slope at best focus.
Optical Pattern Formation
For situations involving large NAs, there is not a single definition for “best focus.” For low-NA optics, where the Rayleigh DOF greatly exceeds the resist thickness, most effects of defocus, such as linewidth and resist-slope variation, behave symmetrically about some plane. Moreover, the smallest features are typically imaged at that plane. In such a circumstance, it is reasonable to define that plane as the plane of best focus. However, for high-NA optics, asymmetry is introduced, and the choice of best focus becomes less obvious. In particular, the middle of the region over which linewidths are within specifications is no longer the place at which the smallest features are resolved, nor the resist slope maximized. Because of the significant effects on lithographic performance, focus needs to be well controlled. Unfortunately, a number of factors can cause focus to vary. For example, a change in barometric pressure can induce a shift in focus. Lenses with glass elements create images by means of the physical phenomenon of refraction where the direction of a beam of light changes at the interface between materials of different indices of refraction. The angle of refraction, and hence the focal distance, depends upon the indices of refraction of the glass and air. While the index of refraction of the air is 1, it differs slightly, and changes as barometric pressure changes. As the air pressure inside of wafer fabricators rises and falls with the outside barometric pressure, the focal length of lenses containing refractive elements also changes.38 The focus adjustment required to keep an exposure tool at best focus while barometric pressure changes for an exposure system that does not have automatic focus for pressure compensation is shown in Fig. 2.33. Modern exposure tools control focus automatically for changes in air pressure. Some systems use pressurized lenses, where the air pressure inside the lens is kept at a fixed value regardless of the pressure of the air in the fab. An alternative method of control involves the measurement of barometric pressure and compensation of the focus through software. In addition to adjusting the focus when barometric pressure changes, exposure tools also need to move wafers up and down, to adjust their tilt, and to correct for changes in wafer thickness and flatness if the resist films are to be maintained in focus. Automatic focusing systems are discussed in detail in Chapter 5. Barometric pressure affects the reduction of the projection optics39 as well as focus, and requires similar compensation. Mirrors with curved surfaces can also be used for imaging. The imaging properties from reflective surfaces are purely geometrical (Fig. 2.34), and are independent of the refractive index of the air or wavelength of the light: I R ,
where ΘI and ΘR are the angles of incidence and reflection, relative to the normal, respectively. Lenses that use mirrors have less sensitivity of focus to barometric pressure than lenses that use only glass elements. Stepper lenses will be discussed in more detail in Chapter 5.
Figure 2.33 Focus correction versus pressure for a stepper equipped with a Zeiss 10-78-46 lens (0.38 NA, g-line).
Figure 2.34 Reflections from mirror lens elements are purely geometrical and independent of the index of refraction of the air.
FLEX (Focus-Latitude Enhancement eXposure) has been proposed as a method for increasing the DOF; this method involves partial exposures at different focus positions.40,41 With FLEX, sharply focused images are superimposed with defocused ones throughout the depth of the resist film. The contact holes are extended by doing partial exposures at multiple locations along the optical axis. FLEX is also known as focus drilling. The appropriate choice of exposure and focus steps can lead to a 3 or 4 increase in contact-hole DOF, but the DOF for line features is typically not improved. FLEX has been demonstrated to improve the DOF but with a loss of ultimate resolution by the multiple defocused exposures.42 As we shall see in Chapter 8, achieving adequate DOF without compromising resolution requires that the fundamental issue of diffraction be addressed.
Optical Pattern Formation
Assuming diffraction-limited optics, show that the optical resolution of a 0.54-NA ArF lens is approximately the same as a 0.7-NA KrF lens. Which has the greater depth-of-focus?
Derive Eq. (2.29).
The following table gives wavelengths and numerical apertures used in volume manufacturing over time: Year 2001 2003 2005 2007
Wavelength 248 nm 193 nm 193 nm 193 nm
NA 0.80 0.75 0.85 0.92
Calculate the Rayleigh DOF for each year. What is the trend for the depthof-focus over time? 2.4
In Fig. 2.18, for a diffraction-limited 0.7-NA lens exposing at a wavelength of 248 nm, the normalized derivatives of the aerial images (image log slopes) at the position of the nominal line edge are as follows: Feature size 250 nm 180 nm 150 nm
Normalized derivative (1/μm) 21.6 17.7 15.0
Using Eq. (2.32), show that the changes in linewidth for a 10% change in exposure dose are 9, 11, and 13 nm for 250-, 180-, and 150-nm features, respectively. Show that the dose control needs to be 27%, 16%, and 11% for 250-, 180-, and 150-nm features, respectively, for linewidths to change by no more than 10% of the feature size. How does the challenge of process control change as smaller features are produced? 2.5
Assuming normally incident coherent light on a grating of equal lines and spaces, show that the angles of incidence onto the wafer of the 1st-order diffracted beams in air are 29.7, 43.5, and 55.8 deg for 250-, 180-, and 150-nm lines, respectively. What are the minimum numerical apertures required to image these features?
Show that the depth-of-focus is reduced by ~59 nm by increasing the resist thickness from 200 nm to 300 nm for a resist with an index of refraction of 1.7.
M. Born and E. Wolf, Principles of Optics, 7th Ed., Cambridge Univ. Press, Cambridge (1999). Note that the sign convention for the angles employed by Born and Wolf (and in this text) is not used universally. As used here, the angles indicated in Fig. 2.5 are positive.
Solid-C was a simulation program produced by SIGMA-C GmbH of Munich, Germany. SIGMA-C was acquired by Synopsys, Inc., in 2006. Synopsys produces lithography simulation software called Sentaurus Lithography™.
G.B. Airy, “On the diffraction of an object-glass with circular aperture,” Trans. Camb. Phil. Soc. 5(3), pp. 283–291 (1835).
Lord Rayleigh, “Investigations in optics, with special reference to the spectroscope,” Phil. Mag. 8, pp. 261–274 (1879).
W.J. Smith, Modern Optical Engineering, 2nd Ed., McGraw Hill, Boston (1990).
W. Oldham, P. Jain, A. Neureuther, C. Ting, and H. Binder, “Contrast in high-performance projection optics,” Proc. Kodak Microelectron. Sem. pp. 75–80 (1981).
J.W. Goodman, Introduction to Fourier Optics, McGraw Hill, New York (1968).
SEMI Standard P19-92, “Specification for metrology pattern cells for integrated circuit manufacture,” Semiconductor Equipment and Materials International (2007).
A.J. den Dekker and A. van den Bos, “Resolution: a survey,” J. Opt. Soc. Am. 14(3), pp. 547–557 (1997).
F. Schellenberg, “Resolution enhancement technology: the past, the present, and extensions for the future,” Proc. SPIE 5377, pp. 1–20 (2004).
H.J. Levinson and W.H. Arnold, “Focus: the critical parameter for submicron lithography,” J. Vac. Sci. Technol. B 5, pp. 293–298 (1987).
W.H. Arnold and H.J. Levinson, “Focus: the critical parameter for submicron lithography, part 2,” Proc. SPIE 772, pp. 21–34 (1987).
L. Larmore, Introduction to Photographic Principles, 2nd Ed., Dover Publications, New York (1965).
P.D. Blais, “Edge acuity and resolution in positive type photoresist systems,” Solid State Technol. 20, 76–85 (1977).
Optical Pattern Formation
W.H. Arnold and H.J. Levinson, “High resolution optical lithography using an optimized single layer photoresist process,” Proc. Kodak Microelectron. Sem. pp. 80–92 (1983).
Shipley Co., Newton, Massachusetts, Private Communication (1996).
H.J. Levinson, unpublished.
Nick Eib, Private Communication (2000).
H.H. Hopkins, Wave Theory of Aberrations, Clarendon Press (1950).
L.E. Stillwagon, R.G. Larson, and G.N. Taylor, “Planarization of substrate topography by spin coating,” J. Electrochem. Soc. 134, 2030– 2037 (1991).
D.B. LaVergne and D.C. Hofer, “Modeling planarization with polymers,” Proc. SPIE 539, pp. 115–122 (1985).
L.K. White, “Approximating spun-on, thin film planarization properties on complex topography,” J. Electrochem. Soc. 132, pp. 168–172 (1985).
H. J. Levinson, Y. Ma, M. Koenig, B. La Fontaine, and R Seltmann, “Proposal for determining exposure latitude requirements.” Proc. SPIE 6924, 69241J (2008).
C. Nölscher, L. Mader, S. Guttenberger, and W. Arden, “Search for the optimum numerical aperture,” Microelectron. Eng. 11, pp. 161–166 (1990).
K. Yamanaka, H. Iwasaki, H. Nozue, and K. Kasama, “NA and σ optimization for high-NA I-line lithography,” Proc. SPIE 1927, pp. 310– 319 (1993).
W.N. Partlo, S.G. Olson, C. Sparkes, and J.E. Connors, “Optimizing NA and sigma for sub-half-micrometer lithography,” Proc. SPIE 1927, pp. 320–331 (1993).
B. Lin, “The optimum numerical aperture for optical projection microlithography,” Proc. SPIE 1463, pp. 42–53, 1991.
A. Suzuki, S. Yabu, and M. Ookubo, “Intelligent optical system of a new stepper,” Proc. SPIE 772, pp. 58–65 (1987).
H. Ohtsuka, K. Abe, Y. Itok and T. Taguchi, “Quantitative evaluation method of conjugate point for practical evaluation of wafer stepper,” Proc. SPIE 1088, pp. 124–133 (1989).
H. Fukuda, A. Imai, T. Terasawa, and S. Okazaki, “New approach to resolution limit and advanced image formation techniques in optical lithography,” IEEE Trans. El. Dev. 38(1), pp. 67–75 (1991).
J.W. Bossung, “Projection printing characterization,” Proc. SPIE 100, pp. 80–84 (1977).
M.S. Yeung, “Modeling high numerical aperture optical lithography,” Proc. SPIE 922, pp. 149–167 (1988).
H.J. Levinson and R. Rice, “Overlay tolerances for VLSI using wafer steppers,” Proc. SPIE 922, pp. 82–93 (1988).
B. Katz, J. Greeneich, M. Bigelow, A. Katz, F. van Hout, and J. Coolsen, “High numerical aperture I-line stepper,” Proc. SPIE 1264, pp. 94–126 (1990).
T.A. Brunner, A.L. Martin, R.M. Martino, C.P. Ausschnitt, T. H. Newman, and M. S. Hibbs, “Quantitative stepper metrology using the focus monitor test mask,” Proc. SPIE 2197, pp. 541–549 (1994).
AZ Electronic Materials, Branchburg, New Jersey (2000).
S.A. Lis, “Processing issues and solutions to conjugate lithography,” Proc. Kodak Microelectron. Sem., pp. 117–136 (1986).
K. Hale and P. Luehrmann, “Consistent image quality in a high performance stepper environment,” Proc. Kodak Microelectron. Sem. pp. 29–46 (1986).
F. Sporon-Fiedler and J. Williams, “Atmospheric pressure induced reduction errors in reduction stepper lenses,” Proc. SPIE 538, pp. 86–90 (1985).
T. Hayashida, H. Fukuda, and N. Hasegawa, “A novel method for improving the defocus tolerance in step-and-repeat photolithography,” Proc. SPIE 772, 66–71 (1987).
H. Fukuda, N. Hasegawa, T. Tanaka, and T. Hayashida, “A new method for enhancing focus latitude in optical lithography: FLEX,” IEEE Electron. Dev. Lett. 8(4), pp. 179–180 (1987).
C.A. Spence, D.C. Cole, and B.B. Peck, “Using multiple focal planes to enhance depth-of-focus,” Proc. SPIE 1674, pp. 285–295 (1992).
Chapter 3 PHOTORESISTS As discussed in Chapter 1, the mask pattern is transferred to the wafer by means of optical projection onto photosensitive materials known as photoresists. These materials clearly play a critical role in lithography. The chemistries of the most common classes of photoresists are outlined in this chapter. However, the emphasis is on operational performance, i.e., the ways in which resists behave, as observable by the practicing lithographer (in contrast to the resist chemist).
3.1 Positive and Negative Resists Resists are broadly classified as positive or negative. Unexposed positive resists normally have very low solubility in developer and become soluble by exposure to light. Negative resists behave in the opposite manner; unexposed negative resists are soluble in developer and lose their solubility upon exposure to light. Negative resists were used predominately prior to the advent of wafer steppers. Resists most widely used in the early years of the semiconductor industry, such as Kodak’s KTFR resist, were based upon the photoinduced cross-linking of low-molecularweight cyclized polyisoprene1,2 (Fig. 3.1). Azide additives were used to improve their sensitivity to light and to facilitate cross-linking (Fig. 3.2). Cross-linking reduced the material’s solubility in organic solvents such as xylene. After exposure, an organic solvent was used to develop the resist by removing the lowmolecular-weight unexposed resist and leaving behind cross-linked, highmolecular-weight material. These early negative resists had a number of deficiencies. During development, the cross-linked material would absorb some of the organic solvent used as the developer, causing swelling. Because of the swelling, closely spaced geometries would come into contact during development and would sometimes remain stuck together, resulting in a patterning defect. This swelling limited the thickness and resolution potential of these resists. The use of organic solvents for developing also created safety and disposal problems that required engineering solutions. The resists were also desensitized when exposed to air because of competing reactions with oxygen that could reduce the amount of cross-linking. The wafers needed to be kept in nitrogen ambient during exposure, complicating exposure tool design.
Figure 3.1 Cyclized polyisoprene.1 53
Figure 3.2 The cross-linking of cyclic polyisoprene, by means of a commonly used azide, 2, 6-bis(4’-azidobenzal)-4-methylcyclohexanone.3,4
With the advent of wafer steppers, the industry shifted to positive photoresists for most critical applications. The earliest commercially available wafer steppers were introduced in the late 1970s with optics that functioned at the mercury g-line (= 436 nm). The negative resists used at that time were not very sensitive at such a long wavelength. There were good reasons to use g-line illumination, such as it facilitated the design and fabrication of the stepper’s projection optics. The mercury g-line is visible (blue) light. Many lens designers were familiar with designing at visible wavelengths, and a great deal of lens metrology involved visual assessment of optical interference patterns. A transition to shorter wavelengths would have required significant development by the lens makers (something that occurred later). Fortunately, there were g-line-sensitive positive resists, based on novolak resins, commercially available at the time steppers were first introduced. This, along with other advantages of the positive resists, resulted in an industry-wide transition from the use of negative resists primarily to the predominant use of positive resists. With the exception of contact-hole patterning (discussed shortly), there were no fundamental reasons that positive resists should have been chosen over negative ones. However, the available positive resists had other necessary attributes, such as the lack of swelling. The transition to positive resists occurred not simply because of intrinsic advantages of positive resists (with the exception of contact-hole patterning), but rather because of specific advantages of the existing (novolak) positive resists relative to the existing (azide/isoprene)
negative resists5 (see Table 3.1). Very-high-resolution negative resists that can be developed in the same aqueous developers as positive resists have been developed,6–8 but the high-resolution negative resists used most commonly today use organic solvent developers. This latter type of resist will be discussed in more detail later in this chapter. In principle, there are no compelling reasons to use positive resists in preference to negative resists, with some exceptions. Consider the aerial image of square features—contact holes—shown in Fig. 3.3. For producing contacts with negative resists, the feature on the mask is a square island of absorber surrounded by glass, while the mask feature for a positive-resist contact process consists of a square of glass surrounded by absorber. As can be seen in Fig. 3.3, the negativeresist process suffers from having undesirable exposure at the center of the contact region, which leads to a risk of closed contacts with low-performing resists. Table 3.1 Properties of azide-negative resists, compared to those of novolakpositive resists.
Azide/isoprene negative resists Swells during development Marginal step coverage Organic solvent developer Toxic strippers Sensitive to ambient oxygen
Novolak resists No swelling during development Good step coverage Aqueous developer Environmentally benign resist strippers Operates well in air
Figure 3.3 Simulated cross sections of the aerial images of 80-nm contact holes. The simulations were performed using the Prolith vector model. The key parameters were wavelength = 193 nm, C-quad illumination, and NA = 1.35. A binary mask was assumed.
The creation of contact holes on wafers was thus facilitated in the early days of lithography by the use of positive resists,9 even though the image-log-slope is larger for the island feature on the mask compared to the hole. Improvements in negative resists enabled engineers to take advantage of the superior image-logslope of the island features. Such improved resists will be discussed later in this chapter. For other patterns, the advantages of one tone of resist over the other are less clear. For example, on a grating with lines and spaces of nearly equal size, the clear and dark patterns are optically a rough equivalent, so one tone of resist is not going to be fundamentally preferable to the other tone. Resists are usually operational over specific wavelength ranges, and they are usually optimized for application at very specific and narrow ranges of wavelength. To work well at a given wavelength, there are several requirements: 1)
The resist photochemistry must take place efficiently. This is important for cost-effective manufacturing, since lengthy times to expose the resists reduce exposure-tool productivity. It should be noted that there is such a thing as an exposure dose that is too low, leading to dose control problems and poor pattern fidelity because of shot noise.10,11 (Shot noise is discussed in Section 3.8 and Chapter 12.)
The resist must not be too optically absorbent. For high-resolution imaging, resist films need to be exposed with a high degree of uniformity from the top of the resist film to the bottom, and light will not penetrate the resist film adequately if it is too optically absorbent.
There must not be competing positive and negative reactions. These can occur when the light drives desired photochemical reactions in a positive resist but may also induce polymer cross-linking, a negative resist characteristic. Such behavior has been observed and is illustrated in Fig. 3.4.12 Shown in this figure are experimental characteristic curves for a resist exposed with KrF and extreme-ultraviolet (EUV) light.
Figure 3.4 Characteristic curves of a single-type resist exposed separately with 248-nm-wavelength and EUV (13.5-nm-wavelength) light.12
(EUV lithography is discussed in detail in Chapter 12.) When exposed with KrF light, the resist shows positive resist characteristics throughout the entire exposure range. On the other hand, with EUV exposure the resist behaves with positive characteristics at low and medium doses, but shows clear negative resist behavior at higher doses. This negative resist behavior has been attributed to cross-linking of the polymers that form the resist. These are some of the broad issues regarding resists. The remainder of this chapter discusses specific technical issues in greater detail.
3.2 Adhesion Promotion Adhesion promotion is required for photoresist to stick to the surfaces of silicon, silicon dioxide, silicon nitride, and many other materials commonly found in semiconductor manufacturing, during resist development and subsequent etches. Silicon-dioxide surfaces are usually covered by a layer of physisorbed water that remains after resist coating if not first removed13 (Fig. 3.5). This adsorbed water layer enables water or solvent to penetrate the interface between the resist and the substrate during resist development, causing a loss of adhesion. An adhesionpromotion process—often referred to as priming—is required to avoid this. The first step in the adhesion-promotion process is dehydration. This is accomplished most frequently by heating the wafers in a vacuum to temperatures typically between 100C and 200C. The wafers are then introduced to a vapor of an adhesion-promoting agent, the most common of which is hexamethyldisilazane, [(CH3)3Si]2NH, usually referred to by its acronym HMDS. This method of priming, where the priming agent is applied by exposing the wafer to a vapor, is referred to as vapor priming. The HMDS forms a film on the surface (Fig. 3.6) to which water does not adhere and prevents developer from undercutting the resist during the development step. HMDS has a vapor pressure of 20 Torr at room temperature, which facilitates its application to the wafer surface. The ambient around the wafers can be reduced to 1 Torr, and then vapor can be introduced from a container of HMDS kept under vacuum. Keeping the HMDS under vacuum has the added advantage of extending its lifetime by avoiding reactions with atmospheric wafer and oxygen, which can lead to HMDS decomposition.14 H
Heat 100o – 200o C
Figure 3.5 Thermal dehydration of a hydrated native oxide on a silicon substrate.
CH3 — Si — CH3
HN — Si — CH3
Figure 3.6 The adhesion-promoting agent, hexamethyldisilazane (HMDS), forms a water-resistant film on the surface of a wafer that prevents developer from undercutting the resist during the development process.
Alternatively, HMDS can be applied by bubbling nitrogen through the HMDS. Maintaining the HMDS under a nitrogen atmosphere also prevents degradation. A likely decomposition reaction for HMDS is [(CH3)3Si]2NH + 2H2O = [(CH3)3Si]2O +NH3, and is very similar to the surface reaction. An ammonia smell is an indicator that the HMDS has degraded. Other materials besides HMDS are used for adhesion promotion, such as trimethylsilyldiethylamine (TMSDEA), N,N-diethylaminotrimethylsilane (DEATS)—[(CH3)3SiN(C2H5)2], or mixtures of DEATS and HMDS. Adhesion to untreated metals is usually not a problem for semiconductor processing, but adhesion promoters are available for use on metals. For metal surfaces, chelating-silane adhesion promoters, such as trimethylsilylacetamide, have been proposed.15,16 The adhesion-promotion process can be monitored by measuring surface wettability. This is usually accomplished by placing a drop of water on a primed wafer and measuring the contact angle (Fig. 3.7). Forces are balanced in equilibrium such that
LV cos SV SL ,
Figure 3.7 A drop of water on a surface.
where γLV is the surface tension of the liquid in equilibrium with its saturated vapor, γSV is the surface tension of the substrate in equilibrium with a saturated atmosphere of water, and γSL is the surface tension between the water and the primed substrate.17 The angle is shown in Fig. 3.7, and a properly primed surface typically has values of 50–70 deg for the contact angle of water. Higher angles indicate greater degrees of priming, i.e., more hydrophobic surfaces and larger values of γSL. From thermodynamic arguments, the work of adhesion of the liquid to the solid has been shown to be18 WA LV 1 cos ,
showing in equation form the greater hydrophobicity associated with larger values of . There is such a thing as over-priming.19 While priming has the positive effect of ensuring resist adhesion during resist development, it often has the effect of reducing the adhesion between the resist and the substrate. That is, the primary purpose of the priming is to prevent liquid from penetrating the resistsubstrate interface during development20 (Fig. 3.8). Large amounts of priming reduce this penetration but may do so at the expense of true adhesion of the resist to the substrate. With over-priming, the resist may not wet the surface of the wafer adequately during the resist-coating operation, resulting in parts of the wafer that are not covered by resist. The resist may delaminate—“pop”—during exposure, because the resist is not adhering adequately to the wafer surface. Vapor priming can be performed in stand-alone priming ovens or in singlewafer modules. With stand-alone ovens, it is possible to bake the wafers for a long time, thereby achieving maximum dehydration. On the other hand, full integration with the rest of the lithography equipment is possible when priming takes place in single-wafer modules. As might be expected, adhesion is a property that is modulated by the resist composition. Some polymers will adhere better to surfaces than others.
Figure 3.8 The penetration of liquid at the interface between resist and the substrate.20
3.3 Resist Spin Coating, Softbake, and Hardbake The equipment and associated recipes for applying photoresist to wafers are critical for ensuring well-controlled lithographic processes. Resist processing will significantly affect linewidth control, but as will be discussed, resist processes can influence overlay control, as well. Moreover, resist processing is typically the primary source of random defects in lithographic processes. Consequently, the operations involved in the processing of resists are very significant determinants of yield. For these reasons, resist processing is very important. Resists as supplied by vendors are typically comprised of materials dissolved in organic solvents, prior to application on wafers. Resist usually is applied to the wafer by a spin coating. In this method, photoresist is dispensed in liquid form onto the wafer (Figs. 3.9 and 3.10). The wafer is then spun about its axis at several hundred to several thousand revolutions per minute (RPM). The resist is subjected
Figure 3.9 Schematic of the process of spin coating. (a) Resist is dispensed onto the wafer in liquid form. (b) The spreading and thinning of resist during spinning.
Figure 3.10 A bare silicon wafer being coated with resist in a DNS RF3 coat module. (Photo courtesy of Dainippon Screen Mfg. Co. Ltd.)21
to centrifugal forces, spreading the resist, and leaving a thin uniform layer adhering to the surface. The faster the spin speed, the thinner the resulting layer of resist (Fig. 3.11). The attractive molecular forces that make the resist viscous reduce the rate of thinning caused by centrifugal forces. Consequently, resists with higher viscosity produce thicker films than resists based on similar chemical platforms but of lower viscosity. The viscosity of resists can be modulated by varying the ratio of solvent and solid materials that compose the resists. As the large centrifugal forces near the edge of the wafer pull on the resist, the attractive molecular forces within the resist pull on resist material near the center of the wafer, where centrifugal forces are smaller. Users select the rate of spin by first determining the final thickness desired. Average thickness can be varied by adjusting the rate of spin and/or resist viscosity. While a coater may be capable of spinning over a wide range of speeds, there is usually a smaller range over which the coatings are uniform. Typically, spinning either too fast or too slow produces nonuniform coatings, as illustrated in Fig. 3.12. Approximate ranges over which uniform coatings are produced are listed in Table 3.2. This range of spinning speed is also somewhat dependent on resist material and solvent. The viscosity of the resist is chosen to provide the desired thickness within the range of spin speed where uniform coatings are obtained. Fine-tuning average resist thickness is accomplished by the final rate of spin. The process of fluid spreading on a spinning disk has been the subject of considerable study since spin coating has emerged as the primary method for applying resists. It is possible to gain insight into the spin-coating process by first considering a simple situation in which a flat wafer (at rest) initially has a uniform layer of fluid at a thickness of h0. It is assumed that the fluid has constant viscosity during the spin-coating process. If the wafer is then spun at a rotation rate of f, starting at time t = 0, then the balance of forces is 24
Figure 3.11 Resist thickness versus spin speed for resists of different viscosities of a family of materials from JSR Micro, Inc. coated on 300-mm-diameter wafers.22
Figure 3.12 Average resist thickness and uniformity of Shin-Etsu 430S resist, coated on 200-mm wafers on an SVG ProCell.23 Table 3.2 Optimum spin speeds for coating photoresist. Wafer diameter (mm) 100 200 300
Range of optimum spin speeds (rpm) 3000–5000 1500–3000 1000–2000
2v 4 2 f 2 r , 2 z
where is the fluid’s viscosity, v is the velocity of material at radial position r and height z, and is the mass density. There is also a conservation-of-mass equation: 2 3 h 4 2 r h , 3 r t
where h is the thickness of the resist at radius r and time t. If any other forces or physical processes are ignored, these equations result in25
h0 162 f 2 2 1 h0 t 3
where the thickness is independent of radius. This equation shows a film that thins to zero thickness as t , while resists tend asymptotically to finite thicknesses.
What is missing from the preceding analysis is solvent evaporation, which causes the viscosity to increase over time to the point where resist solidifies. It is this effect that leads to resist thickness that is fairly independent of spin time, following the initial transient thinning.25 Solvent evaporation causes the resist to cool, thus affecting its viscosity and subsequent rates of evaporation. This evaporation takes place nonuniformly over the wafer surface and is a function of spin speed, exhaust, and solvent type. This variation in solvent evaporation rates can lead to resistthickness nonuniformity. It is possible to compensate for nonuniform rates of solvent evaporation by choosing suitable initial temperatures for the resist, wafer, and ambient atmosphere, which are independently adjustable on modern resist coaters (see Fig. 3.13). Since the resist thickness will depend upon the solvent evaporation, the coating process depends upon the resist’s particular solvent.26 Resist can be dispensed while the wafer is motionless or spinning. These two methods are referred to as static and dynamic dispense, respectively. The dispense nozzle can be held fixed above the center of the wafer during dispense, or, with some hardware configurations, it can be moved. Movable dispense arms are useful for obtaining good resist coatings while using a small amount of photoresist on large-area wafers.
Figure 3.13 Resist uniformity contours as a function of air and resist temperatures for an ArF resist coated on a TEL Lithius Pro-Z track.27 The data are in units of angstroms.
Minimizing resist consumption is important for controlling the cost of lithography because photoresist is expensive. Resists used for noncritical layers can cost as little as $100 per liter, but deep-ultraviolet (DUV) resists (particularly for 193-nm exposures) can cost five times that or more, while resists for emerging technologies can cost as much as $2500 per liter. Since only a small percentage of the dispensed resist actually remains on the wafer after spinning (see Problem 3.1), it is useful to minimize the amount of resist that is actually dispensed. Because of this inefficiency, alternative methods of resist coating, such as the use of microinjectors28 (such as found in ink-jet printers29) or spray coating,30 have been pursued, but the quality of resist coatings produced by these techniques thus far has not justified their adoption for leading-edge lithography. A far more common method for minimizing resist consumption during the resist coating process is surface conditioning by dispensing solvent on the surface of the wafers prior to applying the resist and then spinning the liquid solvent off. This enables uniform and low-defect resist coatings while dispensing smaller volumes of expensive resist or other spin-coated materials.31 The pumps that dispense photoresists are critical components of every resist coater. The pump ensures that defined and reproducible amounts of resist are dispensed onto each wafer. Because it is impossible to produce and package resist that is absolutely defect free, the resist is typically filtered at the point of use, from within the resist pump. When packaged, resists are filtered to levels that are onehalf to one-third of the minimum feature size, which currently represents filtration down to sizes of 10 nm and smaller. Resists are filtered to similar levels at the point of use.32,33 As features become smaller, so do the sizes at which resists are filtered. Because polymer solutions do not pass readily through filters with pore sizes significantly smaller than 50 nm, additional engineering is required to implement point-of-use filtration at very small pore sizes. Regardless, resists and other spincoated materials have been successfully filtered at the point of use with filters with pore sizes smaller than 5 nm. An additional mechanism for removing defects can be introduced by using filter materials that have an affinity for defect-causing constituents in the resist.34-36 Hence, there are two mechanisms for filtering: sieving and adsorption of defects (Fig. 3.14).
Figure 3.14 Illustration of the two mechanisms used for filtering particles from photoresist.36
In addition to particulates, defects in resist films can originate as bubbles in the resist. State-of-the-art pumps must also remove bubbles, which are particularly problematic when new bottles of resist are installed. When high volumes of resist are dispensed rapidly, the pump pulls a significant quantity of resist from the bottle. If the pull on the resist is too great, the resist cavitates, with the resist solvent forming bubbles. This can be avoided by using a suitably-large-diameter tube between the pump and resist bottle. Bubbles can also be pulled into the resist as the pump draws out the last of the resist from the bottle. This can be avoided by installing a new bottle of resist well before the prior one is empty, but this wastes expensive resist. This problem has been addressed with improved fittings for extracting resist that minimizes the amount of resist left in bottles while avoiding bubbles. An alternative type of packaging has also been used, where the resist containers consist of pouches, similar to those used to dispense blood. These pouches are often contained within a bottle37 to ease storage and transport, and to secure the pouches against puncture. Another task that the pump needs to perform in order to avoid defects is suckback. After resist is dispensed, a meniscus of resist will form at the end of the resist nozzle (Fig. 3.15). If the pump does not actively provide some draw on the resist back into the dispense nozzle, a small quantity of resist may drop on the wafer. The suck-back mechanism of the pump prevents this from happening. If the suckback is too large, there is the potential for bubble formation on subsequent dispenses, or the amount of resist dispense may not be well controlled. An optimum amount of suck-back is necessary, dependent upon the viscosity of the resist and the surface tension between the liquid resist and the material of the dispense nozzle. Resists are spun to different thicknesses to satisfy different requirements. The best resolution is often obtained with thin resists (although not necessarily with extremely thin resists); however, resist films need to be thick enough to serve as etch masks or to block ion implantations. High-resolution lithography today typically employs resists with thicknesses of 100 nm or thinner. Very thin coatings
Figure 3.15 Various levels of suck-back in resist dispense nozzles.
Figure 3.16 Substrate topography results in regions with thinner resist than found on flat wafers coated under identical conditions.
had not been used for many years for several reasons, in spite of the resolution potential. First, the resist film needs to be intact throughout the entire etch process, during which the resist film erodes. In typical plasma-etch processes, the etch rate of the resist is less than one-third that of the underlying film but in some instances can have essentially the same etch rate as the substrate film. The resist film must be thick enough to have resist remaining at the end of the etch process over those areas of the substrate that are not supposed to be etched. This includes areas involving substrate topography, where the minimum resist thicknesses often occur.38 A profile of resist over topography is shown schematically in Fig. 3.16. Prior to the widespread use of chemical-mechanical polishing, requirements imposed by wafer topography often determined resist thicknesses. In particular, the resist thickness, as measured in large flat areas, must generally be much thicker than the underlying topography. The impact of asymmetric resist profiles on overlay will be discussed further in Chapter 6. Methods that enable the use of very thin imaging resist layers, even in situations involving underlying topography, are discussed in the last section of this chapter. Besides the problems resulting from substrate topography and etch selectivity, ultrathin resist coatings were long avoided because of concerns with defects, particularly pinholes. Early studies showed large increases in pinhole density for resist coatings thinner than 150 nm.39,40 However, subsequent studies41,42 showed that low-defect ultrathin resist coatings could be obtained by applying the same careful attention to the coating parameters for ultrathin resists that was applied to coating production resists where yields are critical. However, ultrathin resist coatings are fundamentally susceptible to pinhole formation. Insight into the problem was provided by Okoroanyanwu,43 who (referencing earlier work44) showed that the thickness at which instabilities occur in spin-coated films is material-dependent and also depends on the interaction between the liquid resist and the substrate.45
This can be understood as follows. Consider a liquid film of nominal thickness h0 on a flat solid surface. Perturbations in the surface, such as those that arise during spin coating, will induce a pressure gradient.43 At position x and time t, these perturbations induce modulations in the thickness , which are 45 described by sums of terms of the form ,
with amplitude u. The time constant of the perturbation is given by45 1 q2 2 3 A q h0 , 2 h0
where is the fluid’s viscosity, is the surface tension, and A is a materialdependent parameter. For a given wave number q and sufficiently thick film (large values of h0), the time constant is positive, and the waves are damped. However, for films thinner than 1
A 4 , hc 2 2q
the instabilities will grow with time, until the depth of the instability is the same as the nominal resist thickness. At this point, a pinhole forms (Fig. 3.17). Note that the thicknesses at which the instabilities occur are material dependent. Thus, some early observations of pinhole formation were a consequence of intrinsic material properties, not simply the failure to ensure clean coating processes. For future technologies that may require ultrathin resist layers, resists need to be formulated so that they are robust with respect to pinhole formation. Somewhat thick coatings (0.5–3.0 m thick) tend to be required for implant masks, but the resolution required for these layers is usually less than for the most critical layers. Extremely thick coatings, where the thickness can be as thick as 100 m,47 are used for processing thin-film heads for disk drives and for micromachining applications.48,49 The coating of very thick resists involves special considerations. One approach that reduces material consumption and improves uniformity is to use a closed coater bowl which has a solvent-saturated atmosphere.50 This approach is also advantageous for coating square substrates, such as those used for fabricating photomasks, where obtaining good resist uniformity at the corners has always been a challenge.51
Figure 3.17 Critical resist thickness versus wavenumber for polystyrene.46 A = 8 × 10–20 J, and γ = 40 × 10–3 J/m2.
After the resist is dispensed and the wafer has completed its spinning, there is a thick ring of resist at the edge of the wafer referred to as an edge bead.52 The edge bead exists not only on the upper surface of the wafer, but also can exist on the wafer edge. It may even extend to the bottom surface of the wafer, near the wafer edge (Fig. 3.18), and because it can chip and flake, leading to defects, it is desirable to remove the edge bead prior to post-lithographic processing. In the steps that follow lithographic patterning, the wafer may be subjected to elevated temperatures, which will harden the resist and cause the remaining edge bead to be particularly difficult to remove. Consequently, it is best to remove the edge bead during the lithography process. Oftentimes, immediately following resist coat or softbake, the edge bead can be removed by using solvent streams or by exposure. Solvent edge-bead removal is usually applied in the resist-coating module, and the edge bead is typically removed by this method following resist coating. Alternatively, a separate unit may be used to expose the resist at the edge of the wafer, and the edge bead will be removed during the develop step. Optical edgebead removal avoids solvent splashing that can sometimes occur with solvent edge-bead removal. However, there are some films applied by spin coating, such as
Figure 3.18 At the edge of wafers there is extra resist, known as the edge bead.
organic antireflection coatings (to be discussed in Chapter 4), that are not photosensitive, and their edge bead cannot be removed by optical exposure and subsequent develop.53 One of the advantages of coating substrates in a solventsaturated atmosphere is the reduction of the edge bead. Edge-bead removal continues to receive attention. One reason is the highly competitive nature of the semiconductor electronics business, which compels minimizing the width of the edge-bead removal in order to maximize the number of potentially good dies on the wafers. As the width of the edge bead becomes smaller than 2 mm, control requirements become increasingly stringent. The use of immersion lithography, which is discussed in more detail in Chapter 10, injects additional motivation for a high-quality edge-bead-removal process. A novel method for removing edge beads involves the use of pulsed nanosecond to femtosecond lasers at near-UV wavelengths. When used either in air or in conjunction with appropriate gases, edge beads can be removed with good control, and materials that are not typically photosensitive can also be removed. An example of such edge-bead removal is shown in Fig. 3.19. Following coating, the resist film on the wafer usually does not have the desired dissolution properties in developer. For a positive resist, the develop rate of unexposed resist should be very low, but the resist, as coated, is often porous, retains considerable solvent, and has a high develop rate as a consequence. The most common method of densifying the resist is baking. The bake that immediately follows resist coating is referred to as the softbake, pre-bake, or post-apply bake. Several methods of baking resist-coated wafers have been used. Convection ovens were used commonly in the early days of semiconductor processing, but they provided poor consistency and were not amenable to integrated, single-wafer processing. Several other methods were used, including infrared ovens, microwave ovens, and hot plates. Of all the baking methods tried, hot plates have provided the best temperature control, and they are used for all leading edge-resist processing today. On state-of-the-art tools, across-wafer temperature uniformity is > ni, where nj is the refractive index of the reflective layer and ni is the index of refraction of the photoresist.] For a perfectly reflective surface, 100% of the light is reflected and the phase reversal is 180 deg, while light reflected from actual surfaces, which are less-than-perfect reflectors, have magnitudes and phases according to the degree to which the substrates approximate perfect reflectors. All wavelengths of interest to optical lithography are reflected from metals, silicon, and many silicides, so all wavelengths undergo a phase reversal at the resist–reflector interface. For distances on the order of several quarter waves, most wavelengths are still relatively in phase, so the standing waves interfere constructively near the resist–reflector interface. Further away from the interface, the standing waves for different wavelengths will go out of phase.58 For reflective substrates with considerable topography, one of the most egregious problems that result from high reflectivity is that of notching. The problem occurs when there is topography as depicted in Fig. 4.19. Light is reflected from edges and slopes into regions that are intended to be unexposed. This results in notching of resist lines, as shown in Fig. 4.20. It is useful to calculate the distance over which scattered light can be effective in producing notches. Consider the characteristic curve shown in Fig. 2.16. Note that there is negligible resist loss for exposure doses less than some fraction f of E0. Values for f are larger for highercontrast resist, with typical values of 0.7. Wafers typically receive doses Ee that are about twice E0. Notching does not occur as long as the scattered dose Es meets the following condition:
Es fE0 0.7 E0 035Ee .
Figure 4.19 Situation for reflective notching. Light reflects from substrate topography into areas in which exposure is not desired.
Figure 4.20 Example of reflective notching for i-line resist on polysilicon. In the area of the topography the resist is notched. Standing waves resulting from substrate reflectivity are also evident.
The scattered dose at a distance d from a step is given by
E E exp[(d t )] , s e
Modeling and Thin-Film Effects
where is the absorption coefficient for the resist, and t is the resist thickness. From the above two equations, there is no notching so long as e ( d t ) 0.35 ,
where the reflectance from the substrate is . One obvious way to reduce the distance d over which notching may occur is to increase the absorption . This can be done by adding a dye into the resist that does not bleach with exposure, and such an approach has been used extensively.59 The benefit of having dye in the resist was already discussed as a method for reducing the effects of standing waves. There are tradeoffs between absorption to suppress the effects of reflective substrates and image quality. Highly dyed resists have less vertical resist sidewalls, so there is optimum dye loading for resists.60 Values for can be as high as 0.9 for specular aluminum, and a typical value for is 0.6 m–1. For these parameters, no notching occurs for d t 1.5 m . From these considerations, one can see that the utility of dyed resists is small for deep submicron lithography. Moreover, as discussed in the section on photoresists, optical absorption reduces the performance of the resist. Thus far the discussion of antireflection coatings has assumed that the light is normally incident or nearly-normally incident onto the resist. While this is an appropriate approximation to make for imaging at low numerical aperture, it is not suitable for situations involving very high numerical apertures. To understand the complications arising from high angles of incidence, consider the configuration depicted in Fig. 4.21. The effectiveness of a single-layer bottom antireflection coating is shown in Fig. 4.22. At low angles of incidence the antireflection coating is effective, producing nearly the same low reflectance for both S-and Ppolarization. The antireflective coating becomes less effective at larger angles of incidence, and there are substantial differences in behavior between the two types of polarization. Except when imaging simple gratings using S- or P-polarized light,
Figure 4.21 Geometry for light incident on resist.
Figure 4.22 Calculated reflectance of ArF light from a bottom antireflection coating into resist versus the sine of the angle of incidence for light incident on a resist film that is on top of the antireflection coating, all of which is on a silicon substrate.8 The index of refraction and thickness of the antireflection coating are 1.83–0.21i and 135 nm, respectively. The index of refraction of the photoresist is assumed to be 1.8. In some publications, S-polarization is referred to as transverse electric (TE) polarization, while P-polarized light is referred to as transverse magnetic (TM) light.
the inability to produce low reflectance over a large range of angles of incidence is a problem when using lenses with very high numerical apertures, since light will be incident across a wide range of angles. For good process control, low reflectance is required at all angles of incidence. As it turns out, this requires complex antireflection coatings. There are insufficient degrees of freedom to design a single-layer antireflection coating that works across a wide range of angles of incidence. Solutions include antireflection coatings with more than one layer or coatings with indices of refraction that vary through the depth of the film.
4.7 Development For diazonaphthoquinone resists, pattern profiles can be calculated if the development rate R is known as a function of the parameter M (discussed in Sec. 4.3), and the rate is usually measured directly for particular resist and developer systems. Values for M in the resist are simulated using optical models, with suitable modifications as a consequence of diffusion due to post-exposure bakes.
Modeling and Thin-Film Effects
For chemically amplified resists, M can be taken as the fraction of deprotection after post-exposure bake. Development rates are quite nonlinear and are usually fit to particular functional forms in order to facilitate calculations. Various functional forms have been proposed over time. Dill and coworkers proposed the development rate function61 2
Rate e E1 E2 M E3 M .
Other rate functions have since been adopted, notably the “Mack” model:62 Rate rmax
a 1 1 M n a 1 M
where rmax,, rmin, n, and a are parameters of the model. By first calculating M(x,y,z) using imaging models, Eq. (4.44), Eq. (4.45), or a similar equation can then be coupled with a suitable numerical algorithm to complete the simulation of resist profiles.63–65 In this chapter, the major components of pattern formation in resists were discussed in terms of basic physics and chemistry. In the next two chapters, the tools used for exposing wafers and the means for ensuring overlay of successive patterns are discussed in detail. Descriptions are given of specific subsystems— such as lenses and illuminators—that determine some of the parameters that have been discussed thus far.
4.8 Quantum Effects and Modeling The modeling described thus far in this chapter was, for the most part, based on classical physics. As feature sizes become significantly smaller than 50 nm, the quantum nature of the physical world needs to be taken into account for models to be accurate. This quantum character is manifested in several ways. The atomic and molecular structure of materials results in surfaces of features that are not smooth on length scales that are relevant for features that are measured in tens of nanometers, as discussed in Sec. 3.8. Importantly, accurate mathematical descriptions of the lithographic process are no longer deterministic when quantum effects are included in the physical modeling. In such cases, modeling for a given set of process conditions—dose, focus, PEB bake temperature, etc.—will result in an ensemble of predicted resist shapes corresponding to each feature on the mask rather than a single one. This greatly complicates modeling. It should be noted that modeling lithography at the quantum level is currently an active area of research, as the current level of understanding is incomplete.
Models for several key physical processes need to be modified when quantum effects are taken into consideration. First, consider aerial images. The lightintensity profiles created by the methods discussed previously in this chapter are now to be considered as average images. The same is true for light-intensity distributions inside photoresist films, taking into account reflections for substrates. Actual individual images need to account for photon shot noise [Eq. (3.36)]. Similarly, light absorption in the resist film does not occur in the smooth, continuous fashion described by Eq. (4.18). Rather, absorption is a statistical process with a finite probability that photons will be absorbed as they pass through and absorbing medium such as photoresist.66 This was illustrated in Fig. 3.47. The statistical nature of absorption is further manifested when the discrete molecular nature of resist films is taken into account. For optical chemically amplified resists, the most relevant absorption is that by the photoacid generators and photodecomposable bases. In this case, absorption will take place only at specific sites occupied by an absorbing molecule, further distinguishing quantum models from continuum ones. (The situation for EUV resists is more complex and is discussed in Chapter 12.) Diffusion of photoacids and base quenchers is also a phenomenon that can be modeled at the molecular level. These molecules cannot diffuse in any arbitrary direction, but only through interstitial spaces between other molecules comprising the resist film. This is part of the reason that softbake time and temperature have an impact on critical dimensions—higher softbake temperatures and longer times will densify resist films and reduce the free volume, thereby reducing diffusion of photoacids and bases. However, accounting fully for diffusion at the molecular level is complex, and much modeling of post-exposure bakes has deprotection consisting of a blur function centered on points where photoacids are generated.67–70 Current stochastic models typically assume binary states for solubility— soluble or insoluble—based upon the degree of deprotection. Even with this assumption, mesoscale simulations of developed resists have providing insight into the complexity of the development process. As can be seen in Fig. 4.23, some bits of photoresist are not dissolved in the developer because of inadequate deprotection, but rather the resist surrounding these pieces is dissolved, releasing these insoluble pieces from the undissolved remaining resist film. This characteristic contributes to the challenges that have been encountered with controlling the defects in patterns formed in chemically amplified resists. The molecular nature of resist materials also has an impact on the mechanical properties of photoresist that pertain to pattern collapse. Shown in Fig. 4.24 are the results of nanostructure mechanical calculations of the C33 component of the local elasticity matrix. It is notable that the resist features in Fig. 4.24 have an outer layer that has substantially lower rigidity than the bulk material. As features get smaller, the fraction of the volume composed of this lower rigidity material increases,
y position (nm) a)
x position (nm)
x position (nm)
x position (nm)
Modeling and Thin-Film Effects
y position (nm) b)
y position (nm) c)
Figure 4.23 Results of mesoscale simulations of the development of a chemically amplified resist.71
120 nm 40 nm
Figure 4.24 Results of mesoscale simulations of the development of a chemically amplified resist.72
thereby leading to greater susceptibility to pattern collapse as features shrink. That is, for a given type of resist material, the largest aspect ratio that can be sustained without pattern collapse will decrease as features reach sizes at which molecularscale effects become pronounced.
4.9 Summary of Modeling Considerable insight can be gained into the lithographic process by the use of simulation, making modeling an essential tool for all lithographers. Models have varying levels of complexity. The simplest models are accurate for large features and low numerical aperture imaging, but increasingly sophisticated models are required to achieve accuracy for smaller features and with high-resolution optics. Higher accuracy is usually needed with smaller features, if for no other reason than because the tolerable absolute error scales with feature size. For each new node, an assessment of computational accuracy is prudent. There is always a trade-off between computational time and accuracy, so lithographers need to have good physical insight in order to chose the simplest model to use and that will provide sufficient accuracy for the problem at hand. Ultimately, molecular-scale stochastics models are require to achieve the highest accuracy, but these necessarily involve the greatest complexity, as the quantum physics involved is no longer deterministic. Problems of computational time are usually not significant when engineers are trying to simulate the lithographic behavior of individual or small clusters of features, but it will be seen in Chapter 8 that computational efficiency is a significant issue in circumstances where it is necessary to compute the imaging of all features in a chip.
Assume that the index of refraction of the resist is 1.7. For P-polarized light, what is the minimum numerical aperture that is required to produce light rays that have orthogonal polarization in the resist?
Referring to Fig. 4.4, the reflectance for S-polarized light is nearly zero for an angle of incidence of ~60 deg. For what numerical aperture would the most oblique rays have this angle of incidence?
Using the Dill parameters of Table 4.3, show that the light intensity that reaches the bottom of a 1-m-thick film of AZ 1470 resist is 55% and 33% of the incident intensity at the g-line and i-line, respectively, at the very beginning of exposure. Show that these numbers are 97% and 80% for a fully bleached 1-m-thick film of AZ 1470 resist.
Why are post-exposure bakes used for diazonaphthoquinone resists, even though such bakes are not required to complete the photochemical conversion of photoactive compounds?
Modeling and Thin-Film Effects
Suppose that proper exposure of a DNQ resist requires M = 0.1 in the middle of large exposed features. Use Eq. (4.21) to show that an exposure time of 0.15 sec is needed if the value for the Dill parameter A of the resist = 0.8 m–1, B ≈ 0, and C = 0.01 cm2/mJ and the light intensity is 2000 mW/cm2.
Why do bottom antireflection coatings need to absorb light?
For a film with a uniform absorption coefficient and thickness T, show that the amount of light absorbed at the bottom of the film is maximized when
A. Sommerfeld, Optics, Academic Press, New York (1954).
W. Oldham, S. Nandgaonkar, A. Neureuther, and M. O’Toole, “A general simulator for VLSI lithography and etching processes: part I–application to projection lithography,” IEEE Trans. Electr. Dev. ED-26, pp. 717–722 (1980). Most of the work at the University of California at Berkeley for developing lithography simulation was performed by Professors William Oldham and Andrew Neureuther, and their graduate students. In addition to their technical contributions, Profs. Oldham and Neureuther trained many students in lithographic technology, developing our industry’s most important asset – human talent.
C.A. Mack, “Comparison of scalar and vector modeling of image formation in photoresist,” Proc. SPIE 2440, pp. 381–94 (1995).
A. Wong and A. Neureuther, “Examination of polarization and edge effects in photolithographic masks using three-dimensional rigorous simulation,” Proc. SPIE, 2197, pp. 521–527 (1994).
C.A. Mack, “PROLITH: a comprehensive optical lithography model,” Proc. SPIE, 538, pp. 207–220 (1985).
A.R. Neureuther, C. Hsu, T. Horie, J. Cheng, P. Chien, T. James, V. Lee, M. Li, R. Shen, R. Yang, and V. Wien, “Lithography simulation using the Internet,” Microlithography World, pp. 18–20 (Winter, 1999).
D.G. Flagello and A.E. Rosenbluth, “Vector diffraction analysis of phasemask imaging in photoresist films,” Proc. SPIE 1927, pp. 395–412 (1993).
T. Brunner, N. Seong, W. D. Hinsberg, J. A. Hoffnagle, F. A. Houle, and M. I. Sanchez, “High NA lithographic imagery at Brewster’s angle,” Proc. SPIE 4691, pp. 1–10 (2002).
E. Hecht and A. Zajac, Optics, Addison-Wesley, Reading, Massachusetts (1974).
J.E. Gortych and D. Williamson, “Effects of higher-order aberrations on the process window,” Proc. SPIE 1463, pp. 368–381 (1991).
M.S. Yeung, “Measurement of wave-front aberrations in high-resolution optical lithographic systems from printed photoresist patterns,” IEEE Trans. Semi. Manufact. 13(1), pp. 24–33 (2000).
D.G. Flagello, J. de Klerk, G. Davies, R. Rogoff, B. Geh, M. Arnz, Y. Wegmann, and M. Kraemer, “Towards a comprehensive control of full-field image quality in optical photolithography,” Proc. SPIE 3051, pp. 672–686 (1997).
The image intensity contours were provided by Dr. Bernd Geh of Carl Zeiss.
D.G. Flagello and B. Geh, “The influence of lens aberrations in lithography,” Microlithography World, pp. 11–16 (Winter, 1998).
R. Kim and H.J. Levinson, “Application of contrast enhancement layer to 193 nm lithography,” J. Vac. Sci. Technol. B25(6), pp. 2466–2470 (2007).
T. Brunner and R.R. Allen, “In-situ measurement of an image during lithographic exposure,” IEEE Electr. Dev. Lett., EDL-6(7), pp. 329–331 (1985).
T. Brunner and R.R. Allen, “In-situ resolution and overlay measurement on a stepper,” Proc. SPIE 565, pp. 6–13 (1985).
A.K. Pfau, R. Hsu and W.G. Oldham, “A two-dimensional high-resolution stepper image monitor,” Proc. SPIE, 1674, pp. 182–192 (1992).
R.A. Budd, D.B. Dove, J.L. Staples, R.M. Martino, R.A. Ferguson, and J.T. Weed, “Development and application of a new tool for lithographic evaluation, the stepper equivalent aerial image measurement system, AIMS,” IBM J. Res. Dev. 41(12), pp. 119–127 (1997).
A.R. Neureuther, P.K. Jain, and W.G. Oldham, “Factors affecting linewidth control including multiple wavelength exposure and chromatic aberrations,” Proc. SPIE 275, pp. 48–53 (1981).
W.H. Arnold and H.J. Levinson, “High-resolution optical lithography using an optimized single-layer photoresist process,” Proc. Kodak Microelectron. Sem. pp. 80–92 (1983).
Modeling and Thin-Film Effects
J. D. Buckley and . Karatzas. "Step and scan: A systems overview of a new lithography tool," Proc. SPIE Vol. 1088, pp. 424-434 (1989).
M. W. Barrick, D. Bommarito, K. L. Holland, K. C. Norris, B. Patterson, Y. Takamori, J. C. Vigil, and T. J. Wiltshire. "Performance of a 0.5 NA broadband DUV step-and-scan system," Proc. SPIE Vol. 1927, pp. 595608.(1993)
R.W. McCleary, P.J. Tompkins, M.D. Dunn, K.F. Walsh, J.F. Conway, and R.P. Mueller, “Performance of a KrF excimer laser stepper,” Proc. SPIE 922, pp. 396–399 (1988).
F.H. Dill, W.P. Hornberger, P.S. Hauge, and J.M. Shaw, “Characterization of positive photoresist,” IEEE Trans. Electr. Dev. ED-22(7), pp. 445–452 (1975).
Shipley Microelectronics Product Catalog, Shipley Company, Newton, Mass. (1990)
M. Exterkamp, W. Wong, H. Damar, A.R. Neureuther, C.H. Ting, and W.G. Oldham, “Resist characterization: procedures, parameters, and profiles,” Proc. SPIE 334, pp. 182–187 (1982).
Tokyo Ohka, private communication. (2000)
C.A. Mack, “Photoresist process optimization,” Proc. KTI Microelectron. Sem. pp. 153–167 (1987).
H.J. Levinson and W.H. Arnold, “Optical lithography,” Chapter 1 of Handbook of Microlithography, Micromachining and Microfabrication, P. Rai-Choudhury, Ed., SPIE Press, Bellingham, Washington (1997). These equations were derived by Bill Arnold.
C.A. Mack, “Analytical expression for the standing-wave intensity in photoresist,” Appl. Optic. 25, pp. 1958–1961 (1986).
E.J. Walker, “Reduction of photoresist standing-wave effects by postexposure bake,” IEEE Trans. Electr. Dev. ED-22, pp. 464–466 (1975).
T. Batchelder and J. Piatt, “Bake effects in positive photoresist,” Sol. State Technol. pp. 211–217 (August, 1983).
J. Crank, The Mathematics of Diffusion, 2nd Ed., Oxford Univ. Press, Oxford (1975).
D.A. Bernard, “Simulation of post-exposure bake effects on photolithographic performance of a resist film,” Philips J. Res. 42, pp. 566– 582 (1987).
P. Trefonas, B.K. Daniels, M.J. Eller, and A. Zampini, “Examination of the mechanism of the post exposure bake effect,” Proc. SPIE 920, pp. 203–211 (1988).
J. Crank and G.S. Park, Diffusion in Polymers, Academic Press, London (1968).
K. Phan, M. Templeton, and E. Sum, “A systematic approach for i-line manufacturing resist optimization,” Proc. SPIE 1087, pp. 279–289 (1989).
D. Matiut, A. Erdmann, B. Tollkühn, and A. Semmler, “New models for the simulation of post-exposure bake of chemically amplified resists,” Proc. SPIE 5039, pp. 1132–1142 (2003).
S.V. Postnikov, M.D. Stewart, H.V. Tran, M.A. Nierode, D.R. Madeiros, T. Cao, J. Byers, S.E. Webber, and C.G. Willson, “Study of resolution limits due to intrinsic bias in chemically amplified photoresists,” J. Vac. Sci. Technol. B 17(6), pp. 3335–3338 (1999).
B. Tollkühn, A. Erdmann, J. Lammers, C. Nölscher, and A. Semmler, “Do we need complex resist models for predictive simulation of lithographic process performance,” Proc. SPIE 5376, pp. 983–994 (2004).
J. Nakamura, H. Ban, and A. Tanaka, “Influence of acid diffusion on the lithographic performance of chemically amplified resists,” Jpn. J. Appl. Phys. 31, pp. 4294–4300 (1992).
I.I. Bol, “High-resolution optical lithography using dyed single-layer resist,” Proc. Kodak Microelectron. Sem., pp. 19–22 (1984).
C.A. Mack, “Dispelling the myths about dyed photoresist,” Sol. State Technol., pp. 125–130 (January, 1988).
K. Harrison and C. Takemoto, “The use of antireflection coatings for photoresist linewidth control,” Proc. Kodak Microelectron. Sem., pp. 107– 111 (1983).
H. Van den Berg and J. van Staden, “Antireflection coatings on metal layers for photolithographic purposes,” J. Appl. Phys. 50(3), pp. 1212–1214 (1979).
W.H. Arnold, M. Farnaam, and J. Sliwa, “Titanium nitride as an antireflection coating on highly reflective layers for photolithography,” U.S. Patent No. 4,820,611 (1989).
C. Nölscher, L. Mader, and M. Schneegans, “High contrast single layer resists and antireflection layers: an alternative to multilayer resist techniques,” Proc. SPIE 1086, pp. 242–250 (1989).
Modeling and Thin-Film Effects
T. Ogawa, H. Nakano, T. Gocho, T. Tsumori, “SiOxNy:H, high performance antireflection layer for the current and future optical lithography,” Proc. SPIE 2197, pp. 722–732 (1994).
T. Brewer, R. Carlson, and J. Arnold, “The reduction of the standing-wave effects in positive photoresists,” J. Appl. Photogr. Eng. 7(6), pp. 184–186 (1981).
J. Lamb and M.G. Moss, “Expanding photolithography process latitude with organic AR coatings,” Sol. State. Technol., pp. 79–83 (September, 1993).
S. Kaplan, “Linewidth control over topography using a spin-on AR coating,” Proc. KTI Microelectron. Sem., pp. 307–314 (1990).
B. Martin, A.N. Odell, and J.E. Lamb III, “Improved bake latitude organic antireflection coatings for high resolution metalization lithography,” Proc. SPIE 1086, pp. 543–554 (1989).
M. Rocke and M. Schneegans, “Titanium nitride for antireflection control and hillock suppression on aluminum silicon metalization,” J. Vac. Sci. Technol. B 6(4), pp. 1113–1115 (1988).
T. Brunner, “Optimization of optical properties of resist processes,” Proc. SPIE 1466, pp. 297–308 (1991).
T. Tanaka, N. Hasegawa, H. Shiraishi, and S. Okazaki, “A new photolithography technique with antireflection coating on resist: ARCOR,” J. Electrochem. Soc. 137, pp. 3900–3905 (1990).
O.M. Heavens, Optical Properties of Thin Solid Films, Dover, New York (1955).
J. LaRue and C. Ting, “Single and dual wavelength exposure of photoresist,” Proc. SPIE 275, pp. 17–22 (1981).
A.V. Brown and W.H. Arnold, “Optimization of resist optical density for high resolution lithography on reflective surfaces,” Proc. SPIE 539, pp. 259– 266 (1985).
B.K. Daniels and P. Trefonas, “Optimum dye concentration to balance reflective notching against wall angle in positive rhotoresist,” J. Electrochem. Soc. 135(9), pp. 2319–2322 (1988).
F.H. Dill, W.P. Hornberger, P.S. Hauge, and J.M. Shaw, “Characterization of positive rhotoresist,” IEEE Trans. Electr. Dev. ED-22(7), pp. 445–4520 (1975).
C.A. Mack, “Development of positive photoresists,” J. Electrochem. Soc. 134(1), pp. 148–152 (1987).
R.E. Jewett, P.I. Hagouel, A.R. Neureuther, and T. van Duzer, “Line-profile resist development simulation techniques,” Polymer Eng. Sci. 11(6), pp. 381–384 (1977).
J.A. Sethian, “Fast marching level set methods for three-dimensional photolithography development,” Proc. SPIE 2726, pp. 262–272 (1996).
I. Karafyllidis, P.I. Hagouel, A. Thanailakis, and A.R. Neureuther, “An efficient photoresist development simulator based on cellular automata with experimental verification,” IEEE Trans. Semicond. Manufact. 13(1), pp. 61– 75 (2000).
J. C. Slater, Quantum Theory of Matter (2nd ed.). New York: McGrawHill (1968).
G. M. Gallatin, "Continuum model of shot noise and line edge roughness," Proc. SPIE Vol. 4404, pp. 123-133 (2001).
M. D. Smith, "Mechanistic model of line edge roughness," Proc. SPIE Vol.. 6153, p. 61530X (2006).
G. M. Gallatin, P. Naulleau and R. Brainard, “Fundamental limits to EUV photoresist,” Proc. SPIE Vol. 6591, p. 651911 (2007).
R. L Brainard, P. Trefonas, J. H. Lammers, C. A. Cutler, J. F. Mackevich, A. Trefonas, and S. A. Robertson. "Shot noise, LER, and quantum efficiency of EUV photoresists," Proc. SPIE Vol.. 5374, pp. 74-86 (2004).
G. M. Schmid, M. D. Smith, C. A. Mack, V. K. Singh, S. D. Burns, and C. G. Willson. "Understanding molecular-level effects during post-exposure processing," Proc. SPIE Vol. 4345, pp. 1037-1048, (2001).
J. J. De Pablo and F. A. Escobedo. "Molecular simulations in chemical engineering: Present and future." AIChE Journal 48, no. 12, pp. 2716-2721 (2012).
Chapter 5 WAFER STEPPERS AND SCANNERS Wafer steppers and scanners, introduced briefly in Chapter 1, are discussed further in this chapter, paying particular attention to the key subsystems of modern reduction exposure tools, such as light sources, illuminators, reduction lenses, and wafer stages. Alignment systems will be discussed in more detail in Chapter 6. In all of these discussions, the viewpoint will be that of the user.
5.1 Overview Prior to the advent of wafer steppers, circuit patterns were transferred from masks to wafers by contact or proximity printing, or by using full-wafer scanners. In contact printing, a mask that had the pattern for all chips on the wafer was brought into contact with a resist-coated wafer. The mask was illuminated, thereby exposing the resist under the clear features on the mask. This method of exposure was used in the earliest days of the semiconductor electronics industry, but the mechanical contact caused defects on both the mask and wafer, reducing productivity. Proximity printing, where masks and wafers were brought close to each other, but not into contact, was one approach to reducing the problem of defects that arises with contact printing. Unfortunately, resolution was poor when the gap between the mask and the wafer was a practical size, as a consequence of diffraction. The first workable solution to this problem was the full-wafer scanner, which also used a mask that contained the patterns of all chips that were transferred 1:1 to the wafer.1 More detail regarding full-wafer exposure tools is presented in Sec. 5.9. The most common method for making the masks used for contact, proximity, or full-wafer scanning lithography involved a photorepeater.2 The photorepeater had a stage on which an unpatterned mask could be placed and moved precisely (Fig. 5.1). A reduction lens was used to image the pattern of a single chip onto the resist-coated mask blank, exposing the mask one chip at a time and using a precise stage to move the mask between exposures. In order to distinguish between the mask being made with multiple chips and the master object containing the pattern of only one chip, the single-chip mask was called a reticle. Eventually it occurred to someone to eliminate the intermediate mask and exposure tool and essentially use a photorepeater to expose the wafers directly. Thus, the wafer stepper was born. A cutaway view of a wafer stepper is shown in Fig. 5.2. This view shows all the major subsystems (except for the excimer laser light source): reduction lens and illuminator, wafer stage, reticle stage, and wafer-handling cassettes. In the configuration typical of high-performance lithography, resist-processing equipment is interfaced directly to the exposure tool. Resist-coated wafers are 169
taken from the resist-processing equipment and placed by the wafer mechanical handling system on a prealignment station, where the wafers are oriented with respect to the notch (or flat) and centered mechanically. The wafers are then transferred onto a very flat chuck that sits on a stage whose position can be controlled with extreme precision. For optical exposure tools, the wafer is clamped to the chuck with vacuum, while electrostatic clamping is used on EUV exposure tools (Chapter 12). The wafer is exposed while it sits on this chuck. The wafer stage is discussed in more detail later in this chapter.
Figure 5.1 Geometry of the photorepeater.
Figure 5.2 ASML NXT1980i immersion step-and-scan system.
Wafer Steppers and Scanners
Once the wafer is placed on the exposure chuck, it is aligned by automatic systems that detect wafer targets optically and move the stage in small increments to correct the wafer position with respect to the ideal image field. Alignment systems enable the overlay of new patterns to circuit patterns that already exist on the wafer. Prior to exposing each field, the wafer is positioned in the vertical axis by an autofocus system, which in modern steppers also includes the capability to pivot the vacuum chuck that holds the wafer during exposure in order to reduce any net tilt in the wafer surface due to chuck or wafer flatness errors.3,4 Autofocus systems are discussed in more detail later in this chapter. Once the wafer is properly positioned and brought into focus, a shutter in the illumination system is opened, and the resist is exposed in the first exposure field. After exposing the first field, the shutter is closed and the wafer is moved into position to expose the next field. This process is repeated until the entire wafer is exposed. This repetitive process led to the “step-and-repeat” designation for this tool, or “stepper” for short. A similar process, outlined in Chapter 1, takes place when step-and-scan systems are used. The exposed wafer is then moved to an output cassette (or SMIF pod or FOUP) or back to interfaced resist tracks for additional processing. The wafer stepper was introduced commercially in the late 1970s by the GCA Corporation of North Andover, Massachusetts, based on a photorepeater that they were already producing.5 GCA’s first system, the DSW4800, had been preceded by systems designed and built by several semiconductor companies, including Philips, Thomson CSF, and IBM,6–8 who built steppers for their own use and did not sell them commercially. (The Philips stepper technology was eventually commercialized by ASM Lithography.) The DSW in the name of GCA’s stepper referred to “Direct Step on the Wafer,” an allusion to the stepper’s origin in mask making. The GCA DSW4800 stepper, which handled 3-, 4-, or 5-in. wafers, was equipped with a 10× reduction, 0.28-NA, g-line lens that could pattern a maximum square field of 10 10 mm. The lens was supplied by Carl Zeiss of Oberkochen, Germany. The stepper could achieve overlay of +0.7 m (within a fleet of systems) and a resolution of 1.25-m lines and spaces over 1.5-m depth-of-focus. Its list price was about $300,000. Following GCA, several companies began to produce wafer steppers and sell them commercially. The major stepper suppliers today for fine-line patterning are Nikon, Canon, and ASM Lithography (ASML). The GCA operations were absorbed by Ultratech Stepper, which has a significant share of the market for bump and packaging applications. Modern steppers have considerably greater capability than the original GCA DSW4800, but the operating principles are essentially the same. Today, leading-edge systems come in the step-and-scan configuration, while the step-and-repeat format is used for exposures of noncritical layers in semiconductor processing or for applications such as packaging, which typically involve large feature sizes. Chapter 1 lists the defining characteristics of these configurations, and Table 5.1 notes those of contemporary step-and-scan systems in comparison to the DSW4800. Modern systems provide greater overlay and imaging capability than GCA’s first machine. There has also been a substantial improvement in the productivity of exposure tools over time (see Chapter 11).
Table 5.1 Commercially available step-and-scan 193-nm immersion systems, compared to the first commercially available wafer stepper. The relationship between the number of shots (fields) and throughput is discussed further in Chapter 11. Model Lens reduction (N:1) Wavelength (nm) Maximum lens NA Field size (mm)
GCA DSW4800 10× 436 0.28 10 10
Nikon NSR-S631E 4× 193 1.35 26 33
ASML NXT:1980Di 4× 193 1.35 26 33
Overlay, machine-to-itself (nm)
3, 4, 5 in.
Throughput (wafers per hour)
300 mm 300 mm 250 275 20 at 96 fields per at 96 fields per (4-in. wafers) 300-mm wafer 300-mm wafer
5.2 Light Sources As a practical matter, it has proven possible to design lenses that image near the diffraction limit only over narrow bandwidths in wavelength. This is a consequence of the phenomenon of dispersion, where the index of refraction of glass changes with the wavelength of the light. This optical property of glass leads to the well-known phenomenon whereby white light is changed by a prism into a spectrum of separated colors (Fig. 5.3).9 However, there are limits to the range of wavelengths over which lenses can be color corrected while maintaining a practical size and reasonable cost. Consequently, high-resolution stepper lenses image only over a fairly narrow range of wavelengths. Even over the bandwidth of light produced by a line-narrowed laser it is necessary for lens designers to include corrections for the varying optical properties of glass materials over the bandwidth of light. Moreover, intense light sources are needed for cost-effective stepper
Figure 5.3 White light is broken into a spectrum of color by a prism. Typically, the refractive index of glass increases as wavelengths get shorter, increasing refraction for shorter-wavelength light. In lenses, this causes imaging to be wavelength dependent, and compensation for this effect is required in lenses for semiconductor lithography in order to achieve high resolution.
Wafer Steppers and Scanners
throughput, so exposure systems for optical lithography have operated and will continue to operate at wavelengths for which there are intense sources of illumination over narrow bandwidths. This has led to a short list of possible light sources for use in lithography. It should be noted that there are some benefits in this restriction to particular standard wavelengths, since additional technology that depends upon the wavelength is required. For example, resist manufacturers need to develop resists that perform optimally at the specific wavelengths used,10 and pellicles (discussed in Chapter 7) need to be optimized for the specific wavelengths that are used. The limited number of wavelengths at which lithography is practiced enables R&D resources to be well focused. Mercury arc lamps and excimer lasers have been the sources of actinic light for nearly all optical projection photolithography. (Radiation that can induce chemical reactions in photoresists is termed actinic.) The lines of the mercury spectrum and excimer lasing wavelengths used in lithography are listed in Table 5.2. The mercury arc lamp has three intense spectral lines in the blue and ultraviolet portions of the electromagnetic spectrum (Table 5.2), along with some continuum emission in between these spectral lines. The first commercially available wafer stepper, the GCA DSW4800, operated at the mercury g-line, as did the first steppers built by Nikon, Canon, ASML, and TRE (TRE was an early supplier of wafer steppers. They later changed their name to ASET, but discontinued operations in the early 1990s.) These were based upon the same concepts as the GCA DSW4800. The mercury g-line is blue light (λ = 436 nm) in the visible part of the spectrum. As mentioned previously (and to be discussed in more detail in Sec. 5.4), it has proven possible to design stepper lenses that meet the extreme resolution and field size requirements of microlithography only over a very narrow range of wavelengths. For mercury-arc-lamp–based systems, this has been over the bandwidths of the arc lamps on the order of 4–6 nm. These bandwidths are much larger than the natural bandwidths of mercury atomic emissions, because of the collision (pressure) and thermal (Doppler) broadening11 that can be considerable in a high-pressure arc lamp operating at temperatures near 2000C. Some filtering is required for illumination with only the desired spectral line. Table 5.2 Light sources and wavelengths used in optical lithography. Class of light source
Mercury arc lamps
Location in the electromagnetic spectrum
g-line h-line i-line DUV KrF ArF
436 405 365 240–255 248 193
visible visible mid-ultraviolet DUV DUV DUV
Some systems built by Ultratech image over somewhat broader ranges of wavelengths (390–450 nm), but these have resolutions limited to 0.75 m or larger. This use of multiple wavelengths has significant advantages in terms of reducing standing-wave effects,12 and the Ultratech steppers have been used effectively for lithography at 1.0-m feature sizes. Unfortunately, the broadband Ultratech lens design prints the reticle at a 1:1 ratio.13 There is no reduction, and reticle quality has largely prevented the use of Ultratech steppers for critical applications in deep submicron lithography. Besides the lenses from Ultratech, there were a few other lenses that imaged at both the g- and h-line,14 but these had limited acceptance. While the mercury h-line was used on a few wafer steppers,15 most stepper manufacturers made a transition from g-line to i-line lithography in the late 1980s as the need arose to print submicron features, while maintaining depths-of-focus 1.0 m.16 i-line lithography dominated leading-edge lithography until the advent of deep-ultraviolet (DUV) lithography in the mid-1990s. There is a strong band of DUV emission ( = 240 – 255 nm) from mercuryxenon arc lamps, and these were used on early DUV exposure tools, such as the Micrascan I and Micrascan II from SVGL. (SVGL was acquired by ASML in 2001.) Essentially all DUV systems today use excimer lasers as light sources (as did higher-resolution versions of the Micrascan platform17). The bandwidth requirements for these light sources are usually much less than 1.0 picometer (pm). Excimer lasers are considered in more detail, following a discussion of arc lamps. A mercury arc lamp is illustrated in Fig. 5.4. A fused silica bulb is filled through a tip with a small quantity of mercury and argon or mercury and xenon. After filling, the bulb is sealed. Operation is initiated by applying a high-frequency high voltage (>10 kV) across the two electrodes, ionizing the inert gas. The resulting discharge causes the mercury to evaporate, and the mercury begins to contribute to the discharge. The plasma, being electrically conducting, cannot support the high voltage, so the voltage drops, and steady lamp output is maintained by operating the lamp at constant current at relatively low dc voltages (50–150 V). High voltages are needed only to ignite the plasma. Condensation of the mercury to the cooler walls of the bulb near the electrodes is inhibited by reflecting coatings. Pressure inside the bulb can exceed 30 atm during operation,18 and catastrophic failure is always a concern. The electrodes are made of refractory metals, such as tungsten, in order to withstand the internal temperatures that can be as high as 2000C. Thorium coatings are often used to reduce the electrode work functions and provide electrons to the plasma more easily. During operation, electrode material is gradually deposited onto the insides of the bulb, reducing light output. Lamps are usually replaced after several hundred hours of operation in order to maintain high stepper throughput. The probability of a lamp explosion also increases with time, and the prevention of such explosions is another reason why lamps are replaced at the end of their rated lives. The two most common mechanisms of catastrophic failure are degradation of glass–metal seals or fracture of the glass bulb.19
Wafer Steppers and Scanners
Figure 5.4 Mercury arc lamp.
Less than 1% of the electrical power supplied to a mercury arc lamp is converted to actinic light. The rest of the energy is nonactinic light or heat that is removed by air exhaust and cooling water. The air exhaust also serves a safety function, by exhausting mercury vapor in the event of a lamp explosion. Improved stability of light output has also been obtained by monitoring and controlling the external lamp temperature, which will exceed 700C.20 As a practical matter, the lamp base temperature, typically between 150C and 200C, is more easily measured than the bulb temperature. Temperature control is obtained by adjusting the air exhaust. Catastrophic failures can also be avoided by monitors of the voltage and current to the lamp.21 Mercury is a toxic substance, and thorium is radioactive, so both materials present handling and disposal issues. Because thorium is an alpha emitter, it represents no safety hazard to users, as long as the glass bulb is intact. Users of mercury arc lamps need to establish procedures for handling lamp explosions and for the disposal of used arc lamps. Another light source applied to lithography is the excimer laser. Excimer lasers are much larger and more complicated than arc lamps. Because they are so large, and cleanroom floor space is so expensive, excimer lasers are usually placed outside of the cleanroom (Fig. 5.5). The intrinsic directionality of the laser light enables the lasers to be placed up to 25 m away from the stepper, with the light being delivered by a series of mirrors and lenses without a significant loss of light energy. In KrF excimer lasers, excited dimers are created by placing a strong electric field across a gas mixture containing Kr, F2, and Ne.22 A high voltage is used to produce an electrical discharge, which, in turn, drives the reactions that ultimately
Figure 5.5 Configuration for excimer laser light sources, where the lasers are placed far from the stepper.
result in lasing (see Table 5.3).23 Early excimer lasers required voltages >20 kV, and many components failed from high-voltage breakdown.24 Reliability has improved through laser designs that require lower voltages, in the range of 12–15 kV, to produce the electrical discharge, and these lower voltages reduce the stress on all electrical components.25 Excimer lasers produce light in pulses, at rates up to several kilohertz. There has been a transition from thyratron-based discharging electronics to solid-state electronics, and this has also contributed to improvements in laser reliability. Excimer lasers have matured considerably since their first use on commercially available wafer steppers in 198826 to the point where they are sufficiently reliable for industrial use. This improvement in excimer light sources has played a critical role in bringing DUV lithography to production worthiness. To appreciate the degree of reliability required for use in manufacturing, consider that modern KrF and ArF excimer lasers are capable of pulsing at 6 kHz. With a duty factor of only 10%, this represents 18.9 billion pulses a year. Table 5.3 The key reactions in a KrF excimer laser.27
F2 e F F Kr e Kr * e Kr * e Kr 2e
Negative fluorine production Two-step positive krypton production
Kr F Ne KrF * Ne
KrF * Kr F h
KrF * h Kr F 2h
F F Ne F2 Ne
Wafer Steppers and Scanners
The unnarrowed fluorescence spectrum for the KrF* emission is shown in Fig. 5.6.28 There is sufficient gain over only part of this spectrum for lasing, about 400 pm. Freely running ArF lasers have similarly broad bandwidths, with full-width half-maxima of about 450 pm. These bandwidths are much too large for use with all-refractive optics and require narrowing for catadioptric lenses as well. Excimer lasers consist of several subsystems, shown in Fig. 5.7, including linewidth narrowing optics. A high repetition rate is desirable for these pulsed light systems, and excimerlaser suppliers improved the available rates from 200 Hz 29,30 to 4 kHz,31,32 and eventually to 6 kHz.33,34 The higher rates allow for high doses in short times without requiring high-peak light intensities, and this reduces damage to optical elements. Measurements for stepper self-metrology take place no faster than permitted by the excimer-laser frequency, so stepper set-up time is reduced with high-repetition-rate lasers.
Figure 5.6 KrF* fluorescence spectrum.
Figure 5.7 Schematic of a single-chamber excimer laser, showing key subcomponents.
Early excimer lasers produced only a few watts of output power,35 and chemically amplified resists were required to achieve good exposure tool productivity. Excimer lasers for advanced lithography with output powers as high as 120 W have been produced,36 but somewhat lower power (60–90 W) is usually used in practice in order to maintain the exceedingly tight bandwidth requirements of leading-edge optical lithography. Further increases in excimer laser output power are also limited by glass damage that occurs with higher peak power and difficulties in increasing the excimer-laser repetition rate beyond 6 kHz. Glass damage has been a more significant problem with ArF lasers ( = 193 nm) than for KrF lasers ( = 248 nm).37 A high level of atomic fluorine in the discharge region of an excimer laser can cause arcing and other instabilities, so the byproducts from one pulse (see Table 5.3) must be removed from between the electrodes and replenished with fresh gas before another pulse can be fired. The repetition rate is limited by the ability to exchange the gas between the electrodes. Faster exchange rates place significantly greater requirements on fans and motors, with attendant concerns for reliability degradation. Moreover, acoustic waves are generated by each discharge, and these waves reflect from the sidewalls back to the discharge space. The discharge chambers of high repetition rate excimer lasers are designed to minimize these reflections that are relevant at high repetition rates.31,38 In principle, glass damage can be reduced by “stretching” the pulses from their unstretched length of 25–30 nsec,39 reducing the peak energy while maintaining the total-integrated energy.40 Another advantage of temporally longer pulses is a reduction in bandwidth.41 An example of a stretched pulse is shown in Fig. 5.8. Because laser-pulse intensity does not evolve symmetrically in time, temporal pulse length needs definition. The most commonly used definition is the integralsquared pulse width:43
Figure 5.8 Excimer-laser power versus time for a normal and stretched pulse from a Cymer ArF excimer laser.42
Wafer Steppers and Scanners
I t dt . 2 I t dt
This definition is used because this is the pulse duration that is most relevant to the issue of glass damage.43 The requirements for the laser gases cause the cost of installation of excimer laser steppers to increase relative to costs for arc-lamp systems (Table 5.4), particularly since the fluorine gases have safety requirements that must be addressed. An innovative solid source for fluorine addresses this safety issue.44 Since fluorine leads to the etching of silicon dioxide, the windows of the excimer laser are typically made of calcium fluoride, a material that is discussed in more detail in a later section. Laser gases must be very pure, as impurities will cause degradation of laser performance. Since fluorine is a primary excimer laser gas, special materials must be used for handling this very chemically reactive gas. Beam-delivery systems comprise additional expenses associated with excimer-laser steppers that do not exist for arc lamp systems, where the illumination source is built into the stepper. The purpose of the beam-delivery system is to provide an optical path from the excimer laser, which is usually located outside of the cleanroom, to the wafer stepper or scanner. Typically, the beamdelivery system is a set of tubes, containing lenses and mirrors, through which the DUV light traverses the distance between laser and stepper (Fig. 5.5). Performance of the imaging optics requires alignment of the input beam to within 1 deg, positioned to within 150 m,45 while the laser may be separated from the stepper by as much as 25 m. This places tight constraints on tolerable levels of vibration throughout an extended part of the fabricated beam line. Maintaining the 150-m placement of a beam delivered from 10 m away requires 3 arcsec of angular control. A robust way to ensure good alignment of the laser beam is to employ active beam sensing and control of the mirrors in the beam-delivery unit.46 The beam-delivery system must contain optics to address the natural beam divergence of an excimer laser. A laser beam of a cross section 1 2 cm will diverge 5 mrad and 2 mrad, respectively. At a distance of 25 m, the beam spreads to a cross section in excess of 13 6 cm without optics to refocus the beam. The beam-delivery system also typically requires mirrors to bend the beam around Table 5.4 Installation and consumables costs for the illumination systems of arc lamp and excimer laser–based wafer steppers. Availability
Arc lamps 99.5%
KrF excimer lasers 97%
Cost for consumables Installation costs
$40,000/year $1000–$10,000 per stepper
$100,000/year $100,000 per stepper
obstructions between the laser and the stepper. While not as sophisticated as the stepper’s projection optics, the lenses in the beam-delivery system require antireflection coatings to maintain light intensity at the actinic wavelength and also at an optical wavelength, usually 632.8 nm (HeNe laser), for aligning the beamdelivery optics. To avoid photochemically deposited contaminants on the optical elements, the beam-delivery system is enclosed and often purged with nitrogen. Enclosure is also required to provide a Class-1 laser system.47 The lenses and mirrors in beam-delivery units encounter high fluencies, so the lens and mirror coatings need to be resistant to damage by high-intensity light.48 The frequency at which components need to be replaced in order to maintain good performance will depend upon optical-component quality and the level of contamination within the beam-delivery unit. Excimer lasers today are installed and maintained as Class-1 laser systems. This was a critical advance for production environments, where protecting operators from stray DUV light formerly required elaborate shielding walls and curtains during laser installation and maintenance. Stepper manufacturers have responded to this standard of engineering by designing beam-delivery systems that can be aligned while maintaining the systems in Class-1 configurations. Excimer laser utilization has improved relative to the first excimer lasers used for lithography, over and above the improvements resulting from reductions in unscheduled downtime. The gas inside the lasers requires periodic replacement, since small amounts of impurities in the gas reduce lasing efficiency and can deposit coatings on windows. Early excimer lasers for lithography required complete gas refills every 100,000 pulses, while more recent lasers require such refills only every two billion pulses49 or not at all.50 Much of this improvement resulted from the replacement of organic materials, such as Teflon and Viton, with ceramic and pure metal materials for insulators and seals, and improved methods for cleaning parts. Another important innovation was the use of gas injection in small amounts while the laser was in operation.51 Complete gas refills cannot be done while the laser is operating, so refills reduce equipment availability. The use of noble gases has an impact on costs. Krypton is expensive, while helium is nonrenewable.52 Consequently, manufacturers of excimer lasers have made efforts to minimize consumption of these gases.53,54 There have been supply problems with neon because of the limited number of sources, and excimer lasers have been designed to reduce consumption of neon as well.55 There has been a trade-off between gas consumption and laser availability, and the balance has been optimized with some return to the use of gas refills in order to optimize costs by balancing tool availability and noble gas consumption. The step-and-scan configuration places more stringent requirements on the excimer lasers than do step-and-repeat machines. There is a direct relationship between the maximum scan speed and the number of pulses required to achieve a specified dose: H Vm
n , f
Wafer Steppers and Scanners
where H is the slit height in the scan direction, Vm is the maximum wafer-stage scan speed, n is the minimum number of pulses required to achieve the specified dose, and f is the laser repetition rate.56,57 The minimum number of pulses used to achieve the dose is also related to dose control. The standard variation of the dose σD is related to the pulse-to-pulse variation σP–P by
P P n
If σP–P is large, n cannot be too small or there is inadequate dose control. Typical pulse-to-pulse repeatability is about 2.5% (3). Thus, laser pulse-to-pulse variation is directly related to the potential throughput of step-and-scan systems. For example, if 0.1% dose control is required, and the scanner has a slit width of 6 mm and a scan speed of 1 m/sec, then the maximum number of pulses that will expose each feature, according to Eq. (5.2), is 36. This implies a needed pulse-topulse stability [Eq. (5.3)] of 0.6%. A missed pulse, in which the excimer laser simply fails to fire, seriously degrades dose uniformity across the scan, while stepand-repeat systems keep the shutter open for an additional pulse and compensate completely. Thus, greater laser reliability is required for step-and-scan systems than for step-and-repeat systems. Freely running KrF lasers have a natural bandwidth of approximately 300 pm [full-width half-maximum (FWHM)], which is too wide for high-resolution wafer steppers. All-refractive optics require bandwidths of